#------------------------------------------------------------------------------
#$Date: 2020-04-08 03:59:03 +0200 (Wed 08 de Apr de 2020) $
#$Revision: 250477 $
#$URL: svn://www.crystallography.net/cod/cif/7/24/02/7240282.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7240282
loop_
_publ_author_name
'Juillerat, Christian A.'
'Klepov, Vladislav'
'Smith, Mark D.'
'Zur Loye, Hans-Conrad'
_publ_section_title
;
 Targeted Crystal Growth of Uranium Gallophosphates Via the Systematic
 Exploration of the UF4-GaPO4-ACl (A = Cs, Rb) Phase Space
;
_journal_name_full               CrystEngComm
_journal_paper_doi               10.1039/D0CE00343C
_journal_year                    2020
_chemical_formula_moiety         '0.25(O208 P36 Rb44 U32)'
_chemical_formula_sum            'O52 P9 Rb11.02 U8'
_chemical_formula_weight         3957.28
_chemical_name_systematic        Rb11[(UO2)8(PO4)9]
_space_group_crystal_system      tetragonal
_space_group_IT_number           135
_space_group_name_Hall           '-P 4c 2ab'
_space_group_name_H-M_alt        'P 42/m b c'
_atom_sites_solution_primary     dual
_audit_creation_date             2020-01-31
_audit_creation_method
;
Olex2 1.2
(compiled May 18 2018 14:05:52 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2020-02-18 deposited with the CCDC.	2020-04-07 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   25.7697(6)
_cell_length_b                   25.7697(6)
_cell_length_c                   9.3962(2)
_cell_measurement_reflns_used    9908
_cell_measurement_temperature    301(2)
_cell_measurement_theta_max      33.09
_cell_measurement_theta_min      2.50
_cell_volume                     6239.8(2)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      301.14
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0452
_diffrn_reflns_av_unetI/netI     0.0144
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -33
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -33
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            100392
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.500
_diffrn_reflns_theta_min         2.499
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    29.564
_exptl_absorpt_correction_T_max  0.1605
_exptl_absorpt_correction_T_min  0.0668
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016) was used for absorption correction.
wR2(int) was 0.1592 before and 0.0684 after correction.
The Ratio of minimum to maximum transmission is 0.4162.
The λ/2 correction factor is Not present.
;
_exptl_crystal_colour            yellow
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    4.212
_exptl_crystal_description       needle
_exptl_crystal_F_000             6780
_exptl_crystal_preparation       Luminescent
_exptl_crystal_recrystallization_method 'From the Melt'
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.126
_refine_diff_density_min         -1.686
_refine_diff_density_rms         0.266
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.326
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     341
_refine_ls_number_reflns         3807
_refine_ls_number_restraints     32
_refine_ls_restrained_S_all      1.328
_refine_ls_R_factor_all          0.0366
_refine_ls_R_factor_gt           0.0350
_refine_ls_shift/su_max          0.009
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0239P)²+153.3181P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0903
_refine_ls_wR_factor_ref         0.0910
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3640
_reflns_number_total             3807
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d0ce00343c2.cif
_cod_data_source_block           Rb11U8P9O52
_cod_original_cell_volume        6239.8(3)
_cod_database_code               7240282
_shelx_shelxl_version_number     2016/6
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.589
_shelx_estimated_absorpt_t_min   0.156
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(Rb4A) \\sim Ueq, Uanis(Rb4B) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.01
Uanis(O12A) \\sim Ueq, Uanis(O9A) \\sim Ueq, Uanis(O11A) \\sim Ueq: with sigma
of 0.01 and sigma for terminal atoms of 0.01
2. Others
 1*[Sof(Rb5A)]+2*[Sof(Rb5B)]+1*[Sof(Rb5C)]=1 with esd of 0.0001
 2*[Sof(Rb4A)]+1*[Sof(Rb4B)]=0.5 with esd of 0.0001
 Sof(P2B)=Sof(O9B)=Sof(O10B)=Sof(O11B)=Sof(O12B)=1-FVAR(1)
 Sof(P2A)=Sof(O9A)=Sof(O10A)=Sof(O11A)=Sof(O12A)=FVAR(1)
 Sof(P3B)=Sof(O4B)=Sof(O5B)=Sof(O6B)=1-FVAR(2)
 Sof(P3A)=Sof(O4A)=Sof(O5A)=Sof(O6A)=FVAR(2)
 Fixed Sof: U4(0.5) O8(0.5) O15A(0.5) O15B(0.5) O16(0.5) O17(0.5)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z+1/2'
'y, -x, z+1/2'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z-1/2'
'-y, x, -z-1/2'
'x-1/2, -y-1/2, z'
'-x-1/2, y-1/2, z'
'-y-1/2, -x-1/2, z-1/2'
'y-1/2, x-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.43306(2) 0.74606(2) 0.500000 0.01371(11) Uani 1 2 d S T P . .
U2 U 0.26957(2) 0.58312(2) 0.500000 0.01998(12) Uani 1 2 d S T P . .
U3 U 0.11404(2) 0.50708(2) 0.500000 0.01539(11) Uani 1 2 d S T P . .
U4 U 0.23298(3) 0.77002(3) 0.54454(7) 0.01552(14) Uani 0.5 1 d . . . . .
Rb1 Rb 0.10402(5) 0.49348(5) 0.000000 0.0269(3) Uani 1 2 d S T P . .
Rb2 Rb 0.14831(6) 0.64831(6) 0.250000 0.0474(4) Uani 1 2 d S T P . .
Rb3 Rb 0.28578(9) 0.42430(7) 0.500000 0.0570(5) Uani 1 2 d S T P . .
Rb4A Rb 0.4213(2) 0.5896(2) 0.4107(10) 0.0515(17) Uani 0.2159(14) 1 d . U . . .
Rb4B Rb 0.4225(10) 0.5866(10) 0.500000 0.032(5) Uani 0.068(3) 2 d S TU P . .
Rb5A Rb 0.36269(17) 0.86269(17) 0.750000 0.0484(13) Uani 0.471(3) 2 d S T P . .
Rb5B Rb 0.3351(9) 0.8515(7) 0.722(4) 0.049(5) Uani 0.1688(16) 1 d . . . . .
Rb5C Rb 0.3342(10) 0.8342(10) 0.750000 0.054(12) Uani 0.191(3) 2 d S T P . .
Rb6 Rb 0.29981(7) 0.58402(6) 0.000000 0.0494(5) Uani 1 2 d S T P . .
P1 P 0.000000 0.500000 0.250000 0.0138(8) Uani 1 4 d S T P . .
P2A P 0.2145(3) 0.5082(2) 0.2266(10) 0.0145(15) Uani 0.492(15) 1 d . . . . .
P2B P 0.2039(3) 0.5150(2) 0.2850(10) 0.0157(14) Uani 0.508(15) 1 d . . . . .
P3A P 0.3298(5) 0.6804(5) 0.2909(14) 0.0127(19) Uani 0.48(3) 1 d . . . . .
P3B P 0.3197(5) 0.6940(5) 0.3039(13) 0.015(2) Uani 0.52(3) 1 d . . . . .
O1 O 0.4010(4) 0.8086(4) 0.500000 0.026(2) Uani 1 2 d S T P . .
O2 O 0.4686(4) 0.6865(4) 0.500000 0.030(2) Uani 1 2 d S T P . .
O3 O 0.3745(3) 0.7104(4) 0.3483(10) 0.048(2) Uani 1 1 d . . . . .
O4A O 0.2789(6) 0.7131(6) 0.304(2) 0.024(4) Uani 0.48(3) 1 d . . . . .
O4B O 0.2795(7) 0.7246(8) 0.385(2) 0.044(5) Uani 0.52(3) 1 d . . . . .
O5A O 0.3351(5) 0.6748(6) 0.1288(13) 0.016(4) Uani 0.48(3) 1 d . . . . .
O5B O 0.3136(6) 0.7038(7) 0.1462(15) 0.037(5) Uani 0.52(3) 1 d . . . . .
O6A O 0.3239(13) 0.6311(15) 0.370(3) 0.027(6) Uani 0.48(3) 1 d . . . . .
O6B O 0.3135(13) 0.6348(13) 0.326(3) 0.031(6) Uani 0.52(3) 1 d . . . . .
O7 O 0.2175(4) 0.6277(4) 0.500000 0.025(2) Uani 1 2 d S T P . .
O8 O 0.3206(5) 0.5359(5) 0.4643(18) 0.033(6) Uani 0.5 1 d . . . . .
O9A O 0.2486(9) 0.5482(9) 0.292(2) 0.041(5) Uani 0.492(15) 1 d . U . . .
O9B O 0.2329(6) 0.5649(6) 0.2550(19) 0.024(3) Uani 0.508(15) 1 d . . . . .
O10A O 0.2131(5) 0.5142(5) 0.0618(13) 0.017(3) Uani 0.492(15) 1 d . . . . .
O10B O 0.2087(5) 0.5101(4) 0.4519(11) 0.012(3) Uani 0.508(15) 1 d . . . . .
O11A O 0.2376(9) 0.4557(9) 0.247(2) 0.029(5) Uani 0.492(15) 1 d . U . . .
O11B O 0.2278(9) 0.4699(8) 0.214(2) 0.033(5) Uani 0.508(15) 1 d . . . . .
O12A O 0.1577(13) 0.5098(12) 0.282(4) 0.040(8) Uani 0.492(15) 1 d . U . . .
O12B O 0.1465(11) 0.5219(10) 0.263(3) 0.033(6) Uani 0.508(15) 1 d . . . . .
O13 O 0.1078(4) 0.5758(4) 0.500000 0.037(3) Uani 1 2 d S T P . .
O14 O 0.1205(4) 0.4383(4) 0.500000 0.033(3) Uani 1 2 d S T P . .
O15A O 0.0423(9) 0.5053(10) 0.362(3) 0.027(4) Uani 0.5 1 d . . . . .
O15B O 0.0532(10) 0.4943(15) 0.328(3) 0.055(9) Uani 0.5 1 d . . . . .
O16 O 0.1781(5) 0.7269(5) 0.5311(15) 0.025(5) Uani 0.5 1 d . . . . .
O17 O 0.2843(6) 0.8174(6) 0.5615(18) 0.035(3) Uani 0.5 1 d . . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
P2A U1 P2A 88.5(2) 4_565 11_566 ?
O1 U1 P2A 89.6(3) . 4_565 ?
O1 U1 P2A 89.6(3) . 11_566 ?
O1 U1 O3 93.3(4) . . ?
O1 U1 O3 93.3(4) . 10_556 ?
O1 U1 O10A 90.4(4) . 11_566 ?
O1 U1 O10A 90.4(4) . 4_565 ?
O1 U1 O11A 87.4(6) . 11_566 ?
O1 U1 O11A 87.4(6) . 4_565 ?
O1 U1 O11B 85.9(6) . 4_565 ?
O1 U1 O11B 85.9(6) . 11_566 ?
O2 U1 P2A 87.8(3) . 11_566 ?
O2 U1 P2A 87.8(3) . 4_565 ?
O2 U1 O1 176.3(5) . . ?
O2 U1 O3 89.6(4) . . ?
O2 U1 O3 89.6(4) . 10_556 ?
O2 U1 O10A 86.0(4) . 4_565 ?
O2 U1 O10A 86.0(4) . 11_566 ?
O2 U1 O11A 91.5(6) . 4_565 ?
O2 U1 O11A 91.5(6) . 11_566 ?
O2 U1 O11B 92.3(6) . 4_565 ?
O2 U1 O11B 92.3(6) . 11_566 ?
O3 U1 P2A 96.8(3) 10_556 4_565 ?
O3 U1 P2A 96.8(3) . 11_566 ?
O3 U1 P2A 174.0(3) . 4_565 ?
O3 U1 P2A 174.0(3) 10_556 11_566 ?
O3 U1 O3 77.8(5) . 10_556 ?
O3 U1 O10A 127.0(4) 10_556 4_565 ?
O3 U1 O10A 154.7(4) 10_556 11_566 ?
O3 U1 O10A 154.7(4) . 4_565 ?
O3 U1 O10A 127.0(4) . 11_566 ?
O3 U1 O11A 146.0(5) . 4_565 ?
O3 U1 O11A 146.0(5) 10_556 11_566 ?
O3 U1 O11A 68.3(5) . 11_566 ?
O3 U1 O11A 68.3(5) 10_556 4_565 ?
O3 U1 O11B 158.8(6) 10_556 11_566 ?
O3 U1 O11B 81.1(6) 10_556 4_565 ?
O3 U1 O11B 158.8(6) . 4_565 ?
O3 U1 O11B 81.1(6) . 11_566 ?
O10A U1 P2A 58.2(3) 11_566 4_565 ?
O10A U1 P2A 30.3(3) 4_565 4_565 ?
O10A U1 P2A 30.3(3) 11_566 11_566 ?
O10A U1 P2A 58.2(3) 4_565 11_566 ?
O10A U1 O10A 27.9(6) 4_565 11_566 ?
O10A U1 O11A 86.9(6) 11_566 4_565 ?
O10A U1 O11A 59.1(6) 11_566 11_566 ?
O10A U1 O11A 59.1(6) 4_565 4_565 ?
O10A U1 O11A 86.9(6) 4_565 11_566 ?
O11A U1 P2A 28.8(5) 11_566 11_566 ?
O11A U1 P2A 117.1(5) 4_565 11_566 ?
O11A U1 P2A 28.8(5) 4_565 4_565 ?
O11A U1 P2A 117.1(5) 11_566 4_565 ?
O11A U1 O11A 145.6(10) 4_565 11_566 ?
O11B U1 P2A 16.4(5) 11_566 11_566 ?
O11B U1 P2A 16.4(5) 4_565 4_565 ?
O11B U1 P2A 104.4(5) 11_566 4_565 ?
O11B U1 P2A 104.4(5) 4_565 11_566 ?
O11B U1 O10A 74.2(6) 4_565 11_566 ?
O11B U1 O10A 74.2(6) 11_566 4_565 ?
O11B U1 O10A 46.5(6) 11_566 11_566 ?
O11B U1 O10A 46.5(6) 4_565 4_565 ?
O11B U1 O11A 132.7(9) 4_565 11_566 ?
O11B U1 O11A 12.8(5) 11_566 11_566 ?
O11B U1 O11A 12.8(5) 4_565 4_565 ?
O11B U1 O11A 132.7(9) 11_566 4_565 ?
O11B U1 O11B 119.9(10) 4_565 11_566 ?
O6A U2 O6A 66.4(15) . 10_556 ?
O6A U2 O6B 76.6(9) 10_556 . ?
O6A U2 O6B 11.7(9) 10_556 10_556 ?
O6A U2 O6B 11.7(9) . . ?
O6A U2 O6B 76.6(9) . 10_556 ?
O6A U2 O9B 146.6(9) 10_556 . ?
O6A U2 O9B 80.7(8) . . ?
O6A U2 O10B 135.5(9) 10_556 10_556 ?
O6A U2 O10B 135.5(9) . . ?
O6A U2 O10B 155.9(9) . 10_556 ?
O6A U2 O10B 155.9(9) 10_556 . ?
O6B U2 O6B 86.0(14) . 10_556 ?
O6B U2 O9B 154.2(8) 10_556 . ?
O6B U2 O9B 70.1(8) . . ?
O6B U2 O10B 147.4(7) . 10_556 ?
O6B U2 O10B 147.4(7) 10_556 . ?
O6B U2 O10B 126.5(7) 10_556 10_556 ?
O6B U2 O10B 126.5(7) . . ?
O7 U2 O6A 96.7(9) . 10_556 ?
O7 U2 O6A 96.7(9) . . ?
O7 U2 O6B 89.8(8) . . ?
O7 U2 O6B 89.8(8) . 10_556 ?
O7 U2 O8 169.2(5) . 10_556 ?
O7 U2 O8 169.2(5) . . ?
O7 U2 O9A 94.5(7) . 10_556 ?
O7 U2 O9A 94.5(7) . . ?
O7 U2 O9B 80.6(4) . . ?
O7 U2 O10B 90.8(4) . 10_556 ?
O7 U2 O10B 90.8(4) . . ?
O8 U2 O6A 79.4(10) 10_556 10_556 ?
O8 U2 O6A 91.0(9) 10_556 . ?
O8 U2 O6A 79.4(10) . . ?
O8 U2 O6A 91.0(9) . 10_556 ?
O8 U2 O6B 98.9(9) . 10_556 ?
O8 U2 O6B 84.5(9) 10_556 10_556 ?
O8 U2 O6B 84.5(9) . . ?
O8 U2 O6B 98.9(9) 10_556 . ?
O8 U2 O8 21.2(10) 10_556 . ?
O8 U2 O9A 93.9(8) . 10_556 ?
O8 U2 O9A 93.9(8) 10_556 . ?
O8 U2 O9A 75.1(8) . . ?
O8 U2 O9A 75.1(8) 10_556 10_556 ?
O8 U2 O9B 88.8(6) . . ?
O8 U2 O9B 108.2(6) 10_556 . ?
O8 U2 O10B 89.1(5) 10_556 . ?
O8 U2 O10B 85.2(5) . . ?
O8 U2 O10B 85.2(5) 10_556 10_556 ?
O8 U2 O10B 89.1(5) . 10_556 ?
O9A U2 O6A 83.9(10) 10_556 10_556 ?
O9A U2 O6A 149.3(9) 10_556 . ?
O9A U2 O6A 83.9(10) . . ?
O9A U2 O6A 149.3(9) . 10_556 ?
O9A U2 O6B 160.4(9) 10_556 . ?
O9A U2 O6B 160.4(9) . 10_556 ?
O9A U2 O6B 74.9(9) . . ?
O9A U2 O6B 74.9(9) 10_556 10_556 ?
O9A U2 O9A 123.6(11) . 10_556 ?
O9A U2 O9B 14.8(6) . . ?
O9A U2 O9B 129.5(5) 10_556 . ?
O9A U2 O10B 72.6(6) 10_556 . ?
O9A U2 O10B 51.8(6) 10_556 10_556 ?
O9A U2 O10B 51.8(6) . . ?
O9A U2 O10B 72.6(6) . 10_556 ?
O10B U2 O9B 77.9(4) 10_556 . ?
O10B U2 O9B 57.3(4) . . ?
O10B U2 O10B 20.9(5) . 10_556 ?
O10B U3 O10B 21.0(5) 10_556 . ?
O12A U3 O10B 50.7(8) . . ?
O12A U3 O10B 71.7(8) 10_556 . ?
O12A U3 O10B 71.7(8) . 10_556 ?
O12A U3 O10B 50.7(8) 10_556 10_556 ?
O12A U3 O12A 122.4(16) 10_556 . ?
O12A U3 O12B 129.6(7) . 10_556 ?
O12A U3 O12B 129.6(7) 10_556 . ?
O12A U3 O12B 10.9(9) 10_556 10_556 ?
O12A U3 O12B 10.9(9) . . ?
O12B U3 O10B 59.0(7) 10_556 10_556 ?
O12B U3 O10B 79.7(7) 10_556 . ?
O12B U3 O10B 59.0(7) . . ?
O12B U3 O10B 79.7(7) . 10_556 ?
O12B U3 O12B 135.1(15) 10_556 . ?
O13 U3 O10B 93.3(4) . 10_556 ?
O13 U3 O10B 93.3(4) . . ?
O13 U3 O12A 90.8(8) . . ?
O13 U3 O12A 90.8(8) . 10_556 ?
O13 U3 O12B 82.8(6) . . ?
O13 U3 O12B 82.8(6) . 10_556 ?
O13 U3 O14 179.8(5) . . ?
O13 U3 O15A 86.9(7) . . ?
O13 U3 O15A 86.9(7) . 10_556 ?
O13 U3 O15B 94.7(10) . . ?
O13 U3 O15B 94.7(10) . 10_556 ?
O14 U3 O10B 86.5(4) . 10_556 ?
O14 U3 O10B 86.5(4) . . ?
O14 U3 O12A 89.2(8) . . ?
O14 U3 O12A 89.2(8) . 10_556 ?
O14 U3 O12B 97.2(6) . . ?
O14 U3 O12B 97.2(6) . 10_556 ?
O14 U3 O15A 93.2(7) . 10_556 ?
O14 U3 O15A 93.2(7) . . ?
O14 U3 O15B 85.4(10) . . ?
O14 U3 O15B 85.4(10) . 10_556 ?
O15A U3 O10B 134.5(6) 10_556 10_556 ?
O15A U3 O10B 155.5(6) 10_556 . ?
O15A U3 O10B 134.5(6) . . ?
O15A U3 O10B 155.5(6) . 10_556 ?
O15A U3 O12A 83.8(10) 10_556 10_556 ?
O15A U3 O12A 153.8(9) . 10_556 ?
O15A U3 O12A 153.8(9) 10_556 . ?
O15A U3 O12A 83.8(10) . . ?
O15A U3 O12B 76.0(9) . . ?
O15A U3 O12B 144.9(8) 10_556 . ?
O15A U3 O12B 144.9(8) . 10_556 ?
O15A U3 O12B 76.0(9) 10_556 10_556 ?
O15A U3 O15A 70.0(11) . 10_556 ?
O15A U3 O15B 80.9(7) 10_556 . ?
O15A U3 O15B 13.0(6) 10_556 10_556 ?
O15A U3 O15B 13.0(6) . . ?
O15A U3 O15B 80.9(7) . 10_556 ?
O15B U3 O10B 144.1(6) . 10_556 ?
O15B U3 O10B 123.5(6) 10_556 10_556 ?
O15B U3 O10B 144.1(6) 10_556 . ?
O15B U3 O10B 123.5(6) . . ?
O15B U3 O12A 73.3(10) 10_556 10_556 ?
O15B U3 O12A 163.4(12) 10_556 . ?
O15B U3 O12A 163.4(12) . 10_556 ?
O15B U3 O12A 73.3(10) . . ?
O15B U3 O12B 66.7(10) 10_556 10_556 ?
O15B U3 O12B 156.8(9) 10_556 . ?
O15B U3 O12B 66.7(10) . . ?
O15B U3 O12B 156.8(9) . 10_556 ?
O15B U3 O15B 90.6(14) 10_556 . ?
U4 U4 O4A 127.0(4) 10_556 10_556 ?
U4 U4 O4A 167.1(4) 10_556 16_566 ?
U4 U4 O4B 48.1(4) 10_556 . ?
U4 U4 O4B 111.7(6) 10_556 10_556 ?
U4 U4 O5A 109.4(3) 10_556 16_566 ?
U4 U4 O5B 125.2(6) 10_556 16_566 ?
U4 U4 O5B 37.0(4) 10_556 7_455 ?
U4 U4 O16 68.4(4) 10_556 10_556 ?
U4 U4 O16 86.0(5) 10_556 . ?
U4 U4 O17 95.1(5) 10_556 . ?
U4 U4 O17 61.0(5) 10_556 10_556 ?
O4A U4 O4A 64.7(6) 10_556 16_566 ?
O4A U4 O5A 123.6(5) 10_556 16_566 ?
O4B U4 O4A 143.8(6) . 16_566 ?
O4B U4 O4A 80.5(6) 10_556 16_566 ?
O4B U4 O4A 79.1(6) . 10_556 ?
O4B U4 O4A 16.4(7) 10_556 10_556 ?
O4B U4 O4B 63.6(10) 10_556 . ?
O4B U4 O5A 138.7(6) 10_556 16_566 ?
O4B U4 O5A 157.3(5) . 16_566 ?
O4B U4 O5B 147.4(8) 10_556 7_455 ?
O4B U4 O16 98.5(8) 10_556 . ?
O4B U4 O16 104.5(7) 10_556 10_556 ?
O4B U4 O17 85.3(8) 10_556 . ?
O4B U4 O17 97.8(9) 10_556 10_556 ?
O5A U4 O4A 58.9(4) 16_566 16_566 ?
O5B U4 O4A 44.2(6) 16_566 16_566 ?
O5B U4 O4A 107.6(7) 16_566 10_556 ?
O5B U4 O4A 131.6(6) 7_455 16_566 ?
O5B U4 O4A 163.6(7) 7_455 10_556 ?
O5B U4 O4B 168.5(8) 16_566 . ?
O5B U4 O4B 122.0(7) 16_566 10_556 ?
O5B U4 O4B 84.6(6) 7_455 . ?
O5B U4 O5A 17.3(6) 16_566 16_566 ?
O5B U4 O5A 72.7(6) 7_455 16_566 ?
O5B U4 O5B 88.2(10) 16_566 7_455 ?
O5B U4 O16 95.9(8) 16_566 . ?
O5B U4 O16 105.6(8) 16_566 10_556 ?
O5B U4 O17 99.7(8) 16_566 10_556 ?
O5B U4 O17 79.8(8) 16_566 . ?
O16 U4 O4A 88.0(6) . 16_566 ?
O16 U4 O4A 103.4(5) 10_556 10_556 ?
O16 U4 O4A 105.1(6) 10_556 16_566 ?
O16 U4 O4A 93.0(6) . 10_556 ?
O16 U4 O4B 92.9(7) . . ?
O16 U4 O4B 81.2(7) 10_556 . ?
O16 U4 O5A 87.9(5) . 16_566 ?
O16 U4 O5A 93.8(5) 10_556 16_566 ?
O16 U4 O5B 75.5(6) 10_556 7_455 ?
O16 U4 O5B 89.4(6) . 7_455 ?
O16 U4 O16 17.5(9) . 10_556 ?
O16 U4 O17 146.7(6) . 10_556 ?
O16 U4 O17 175.3(6) . . ?
O16 U4 O17 129.3(6) 10_556 10_556 ?
O17 U4 O4A 90.1(6) . 16_566 ?
O17 U4 O4A 90.0(6) . 10_556 ?
O17 U4 O4A 109.7(6) 10_556 10_556 ?
O17 U4 O4A 123.3(6) 10_556 16_566 ?
O17 U4 O4B 69.0(7) 10_556 . ?
O17 U4 O4B 91.1(8) . . ?
O17 U4 O5A 98.5(5) 10_556 16_566 ?
O17 U4 O5A 87.5(6) . 16_566 ?
O17 U4 O5B 88.7(7) . 7_455 ?
O17 U4 O5B 62.1(7) 10_556 7_455 ?
O17 U4 O16 162.9(7) . 10_556 ?
O17 U4 O17 34.0(10) . 10_556 ?
O10A Rb1 O10A 23.0(5) 10 . ?
O10A Rb1 O12A 73.0(7) . 10 ?
O10A Rb1 O12A 50.1(7) 10 10 ?
O10A Rb1 O12A 50.1(7) . . ?
O10A Rb1 O12A 73.0(7) 10 . ?
O10A Rb1 O13 93.0(3) 10 7_455 ?
O10A Rb1 O13 93.0(3) . 7_455 ?
O10A Rb1 O14 120.5(3) . 15_665 ?
O10A Rb1 O14 120.5(3) 10 15_665 ?
O10A Rb1 O15A 144.2(5) 10 15_665 ?
O10A Rb1 O15A 166.0(4) 10 8 ?
O10A Rb1 O15A 128.9(5) 10 16_565 ?
O10A Rb1 O15A 142.5(5) . 16_565 ?
O10A Rb1 O15A 166.0(4) . 15_665 ?
O10A Rb1 O15A 142.5(5) 10 7_455 ?
O10A Rb1 O15A 144.2(5) . 8 ?
O10A Rb1 O15A 128.9(5) . 7_455 ?
O12A Rb1 O12A 122.7(13) 10 . ?
O12A Rb1 O13 88.5(6) 10 7_455 ?
O12A Rb1 O13 88.5(6) . 7_455 ?
O12A Rb1 O14 106.9(6) . 15_665 ?
O12A Rb1 O14 106.9(6) 10 15_665 ?
O12A Rb1 O15A 95.0(8) . 8 ?
O12A Rb1 O15A 142.2(8) . 15_665 ?
O12A Rb1 O15A 87.3(7) 10 16_565 ?
O12A Rb1 O15A 133.0(7) . 16_565 ?
O12A Rb1 O15A 95.0(8) 10 15_665 ?
O12A Rb1 O15A 133.0(7) 10 7_455 ?
O12A Rb1 O15A 142.2(8) 10 8 ?
O12A Rb1 O15A 87.3(7) . 7_455 ?
O12B Rb1 O10A 75.6(6) . 10 ?
O12B Rb1 O10A 75.6(6) 10 . ?
O12B Rb1 O10A 53.2(6) 10 10 ?
O12B Rb1 O10A 53.2(6) . . ?
O12B Rb1 O12A 124.0(4) 10 . ?
O12B Rb1 O12A 8.0(8) . . ?
O12B Rb1 O12A 8.0(8) 10 10 ?
O12B Rb1 O12A 124.0(4) . 10 ?
O12B Rb1 O12B 124.0(11) . 10 ?
O12B Rb1 O13 80.8(5) 10 7_455 ?
O12B Rb1 O13 80.8(5) . 7_455 ?
O12B Rb1 O14 112.4(5) 10 15_665 ?
O12B Rb1 O14 112.4(5) . 15_665 ?
O12B Rb1 O15A 140.2(7) . 15_665 ?
O12B Rb1 O15A 125.4(7) . 16_565 ?
O12B Rb1 O15A 81.2(7) . 7_455 ?
O12B Rb1 O15A 93.5(7) 10 15_665 ?
O12B Rb1 O15A 81.2(7) 10 16_565 ?
O12B Rb1 O15A 125.4(7) 10 7_455 ?
O12B Rb1 O15A 140.2(7) 10 8 ?
O12B Rb1 O15A 93.5(7) . 8 ?
O13 Rb1 O14 145.8(3) 7_455 15_665 ?
O13 Rb1 O15A 93.9(4) 7_455 15_665 ?
O13 Rb1 O15A 93.9(4) 7_455 8 ?
O13 Rb1 O15A 54.0(5) 7_455 7_455 ?
O13 Rb1 O15A 54.0(5) 7_455 16_565 ?
O14 Rb1 O15A 55.2(5) 15_665 15_665 ?
O14 Rb1 O15A 55.2(5) 15_665 8 ?
O15A Rb1 O14 95.4(5) 16_565 15_665 ?
O15A Rb1 O14 95.4(5) 7_455 15_665 ?
O15A Rb1 O15A 49.1(9) 16_565 7_455 ?
O15A Rb1 O15A 40.4(9) 16_565 15_665 ?
O15A Rb1 O15A 47.2(8) 15_665 8 ?
O15A Rb1 O15A 64.6(6) 7_455 15_665 ?
O15A Rb1 O15A 64.6(6) 16_565 8 ?
O15A Rb1 O15A 40.4(9) 7_455 8 ?
O7 Rb2 O7 145.6(4) 7_455 . ?
O7 Rb2 O9B 55.9(4) . . ?
O7 Rb2 O9B 123.8(4) . 7_455 ?
O7 Rb2 O9B 55.9(4) 7_455 7_455 ?
O7 Rb2 O9B 123.8(4) 7_455 . ?
O7 Rb2 O12B 128.5(5) 7_455 . ?
O7 Rb2 O12B 128.5(5) . 7_455 ?
O7 Rb2 O12B 78.5(6) 7_455 7_455 ?
O7 Rb2 O12B 78.5(6) . . ?
O7 Rb2 O13 60.8(2) 7_455 7_455 ?
O7 Rb2 O13 150.6(3) 7_455 . ?
O7 Rb2 O13 150.6(3) . 7_455 ?
O7 Rb2 O13 60.8(2) . . ?
O7 Rb2 O16 50.6(3) 7_455 7_455 ?
O7 Rb2 O16 107.0(3) 7_455 . ?
O7 Rb2 O16 50.6(3) . . ?
O7 Rb2 O16 107.0(3) . 7_455 ?
O9B Rb2 O9B 179.1(6) . 7_455 ?
O9B Rb2 O12B 134.6(6) . 7_455 ?
O9B Rb2 O12B 46.2(6) . . ?
O9B Rb2 O12B 46.2(6) 7_455 7_455 ?
O9B Rb2 O12B 134.6(6) 7_455 . ?
O9B Rb2 O13 101.5(4) . 7_455 ?
O9B Rb2 O13 79.1(4) . . ?
O9B Rb2 O13 79.1(4) 7_455 7_455 ?
O9B Rb2 O13 101.5(4) 7_455 . ?
O9B Rb2 O16 75.3(4) 7_455 . ?
O9B Rb2 O16 104.1(4) 7_455 7_455 ?
O9B Rb2 O16 104.1(4) . . ?
O9B Rb2 O16 75.3(4) . 7_455 ?
O12B Rb2 O12B 88.5(10) 7_455 . ?
O12B Rb2 O16 105.2(5) . 7_455 ?
O12B Rb2 O16 124.5(6) 7_455 7_455 ?
O12B Rb2 O16 105.2(5) 7_455 . ?
O12B Rb2 O16 124.5(6) . . ?
O13 Rb2 O12B 51.6(5) 7_455 7_455 ?
O13 Rb2 O12B 72.1(6) 7_455 . ?
O13 Rb2 O12B 72.1(6) . 7_455 ?
O13 Rb2 O12B 51.6(5) . . ?
O13 Rb2 O13 99.2(3) 7_455 . ?
O13 Rb2 O16 81.4(3) 7_455 7_455 ?
O13 Rb2 O16 153.9(3) . 7_455 ?
O13 Rb2 O16 154.0(3) 7_455 . ?
O13 Rb2 O16 81.4(3) . . ?
O16 Rb2 O7 55.1(3) 10_556 . ?
O16 Rb2 O7 100.5(3) 10_556 7_455 ?
O16 Rb2 O7 100.5(3) 16_565 . ?
O16 Rb2 O7 55.1(3) 16_565 7_455 ?
O16 Rb2 O9B 73.0(4) 16_565 . ?
O16 Rb2 O9B 106.4(4) 16_565 7_455 ?
O16 Rb2 O9B 106.4(4) 10_556 . ?
O16 Rb2 O9B 73.0(4) 10_556 7_455 ?
O16 Rb2 O12B 130.9(6) 16_565 7_455 ?
O16 Rb2 O12B 130.9(6) 10_556 . ?
O16 Rb2 O12B 107.0(5) 16_565 . ?
O16 Rb2 O12B 107.0(5) 10_556 7_455 ?
O16 Rb2 O13 152.0(3) 10_556 7_455 ?
O16 Rb2 O13 152.0(3) 16_565 . ?
O16 Rb2 O13 88.5(3) 16_565 7_455 ?
O16 Rb2 O13 88.5(3) 10_556 . ?
O16 Rb2 O16 109.4(4) 7_455 . ?
O16 Rb2 O16 97.3(5) 10_556 16_565 ?
O16 Rb2 O16 103.2(4) 10_556 7_455 ?
O16 Rb2 O16 103.2(4) 16_565 . ?
O16 Rb2 O16 7.1(4) 16_565 7_455 ?
O16 Rb2 O16 7.1(4) 10_556 . ?
O5A Rb3 O5A 51.4(5) 12_656 3_655 ?
O5A Rb3 O5B 16.6(4) 12_656 12_656 ?
O5A Rb3 O5B 16.6(4) 3_655 3_655 ?
O5A Rb3 O5B 54.4(4) 12_656 3_655 ?
O5A Rb3 O5B 54.4(4) 3_655 12_656 ?
O5A Rb3 O8 136.2(4) 3_655 . ?
O5A Rb3 O8 128.7(4) 12_656 . ?
O5A Rb3 O8 128.7(4) 3_655 10_556 ?
O5A Rb3 O8 136.2(4) 12_656 10_556 ?
O5A Rb3 O10B 155.8(4) 12_656 10_556 ?
O5A Rb3 O10B 155.8(4) 3_655 . ?
O5A Rb3 O10B 141.4(3) 12_656 . ?
O5A Rb3 O10B 141.4(3) 3_655 10_556 ?
O5A Rb3 O11A 140.1(5) 3_655 . ?
O5A Rb3 O11A 91.7(5) 3_655 10_556 ?
O5A Rb3 O11A 91.7(5) 12_656 . ?
O5A Rb3 O11A 140.1(5) 12_656 10_556 ?
O5A Rb3 O11B 144.5(4) 12_656 10_556 ?
O5A Rb3 O11B 96.0(4) 12_656 . ?
O5A Rb3 O11B 144.5(4) 3_655 . ?
O5A Rb3 O11B 96.0(4) 3_655 10_556 ?
O5B Rb3 O5B 51.3(5) 12_656 3_655 ?
O5B Rb3 O11B 90.3(5) 3_655 10_556 ?
O5B Rb3 O11B 135.4(5) 12_656 10_556 ?
O5B Rb3 O11B 90.3(5) 12_656 . ?
O5B Rb3 O11B 135.4(5) 3_655 . ?
O8 Rb3 O5B 141.1(4) 10_556 3_655 ?
O8 Rb3 O5B 141.1(4) . 12_656 ?
O8 Rb3 O5B 151.0(4) . 3_655 ?
O8 Rb3 O5B 151.0(4) 10_556 12_656 ?
O8 Rb3 O8 12.7(6) 10_556 . ?
O8 Rb3 O11B 72.9(5) . . ?
O8 Rb3 O11B 83.5(5) 10_556 . ?
O8 Rb3 O11B 83.5(5) . 10_556 ?
O8 Rb3 O11B 72.9(5) 10_556 10_556 ?
O10B Rb3 O5B 141.4(4) . 3_655 ?
O10B Rb3 O5B 130.6(4) 10_556 3_655 ?
O10B Rb3 O5B 130.6(4) . 12_656 ?
O10B Rb3 O5B 141.4(4) 10_556 12_656 ?
O10B Rb3 O8 58.7(3) . . ?
O10B Rb3 O8 60.9(3) 10_556 . ?
O10B Rb3 O8 60.9(3) . 10_556 ?
O10B Rb3 O8 58.7(3) 10_556 10_556 ?
O10B Rb3 O10B 17.3(4) . 10_556 ?
O10B Rb3 O11B 63.9(4) 10_556 . ?
O10B Rb3 O11B 63.9(4) . 10_556 ?
O10B Rb3 O11B 46.8(4) 10_556 10_556 ?
O10B Rb3 O11B 46.8(4) . . ?
O11A Rb3 O5B 85.9(5) . 12_656 ?
O11A Rb3 O5B 131.6(5) 10_556 12_656 ?
O11A Rb3 O5B 131.6(5) . 3_655 ?
O11A Rb3 O5B 85.9(5) 10_556 3_655 ?
O11A Rb3 O8 76.3(6) . . ?
O11A Rb3 O8 76.3(6) 10_556 10_556 ?
O11A Rb3 O8 87.2(6) . 10_556 ?
O11A Rb3 O8 87.2(6) 10_556 . ?
O11A Rb3 O10B 50.8(5) 10_556 10_556 ?
O11A Rb3 O10B 50.8(5) . . ?
O11A Rb3 O10B 67.9(5) . 10_556 ?
O11A Rb3 O10B 67.9(5) 10_556 . ?
O11A Rb3 O11A 116.2(9) . 10_556 ?
O11A Rb3 O11B 4.4(7) 10_556 10_556 ?
O11A Rb3 O11B 4.4(7) . . ?
O11A Rb3 O11B 112.9(4) . 10_556 ?
O11A Rb3 O11B 112.9(4) 10_556 . ?
O11B Rb3 O11B 109.5(7) 10_556 . ?
Rb4A Rb4A U2 77.90(12) 10_556 . ?
Rb4A Rb4A P3A 108.7(3) 10_556 . ?
Rb4A Rb4A P3B 105.0(2) 10_556 . ?
Rb4A Rb4A O2 73.20(19) 10_556 . ?
Rb4A Rb4A O3 100.0(2) 10_556 . ?
Rb4A Rb4A O6A 52.9(6) 10_556 10_556 ?
Rb4A Rb4A O6A 98.0(6) 10_556 . ?
Rb4A Rb4A O6B 104.7(5) 10_556 . ?
Rb4A Rb4A O8 68.2(3) 10_556 10_556 ?
Rb4A Rb4A O8 80.3(4) 10_556 . ?
Rb4B Rb4A U2 79.8(19) . . ?
Rb4B Rb4A Rb4A 6(2) . 10_556 ?
Rb4B Rb4A P3A 114(2) . . ?
Rb4B Rb4A P3B 110(2) . . ?
Rb4B Rb4A O2 77.0(17) . . ?
Rb4B Rb4A O3 106(2) . . ?
Rb4B Rb4A O6A 57(2) . 10_556 ?
Rb4B Rb4A O6A 102(2) . . ?
Rb4B Rb4A O6B 109(2) . . ?
Rb4B Rb4A O8 79.7(17) . . ?
Rb4B Rb4A O8 67.7(17) . 10_556 ?
P3A Rb4A U2 55.8(2) . . ?
P3A Rb4A P3B 3.9(3) . . ?
P3B Rb4A U2 54.9(2) . . ?
O2 Rb4A U2 112.7(3) . . ?
O2 Rb4A P3A 78.5(3) . . ?
O2 Rb4A P3B 76.2(3) . . ?
O2 Rb4A O3 53.8(3) . . ?
O2 Rb4A O6A 82.2(7) . 10_556 ?
O2 Rb4A O6B 97.2(7) . . ?
O2 Rb4A O8 135.6(4) . . ?
O2 Rb4A O8 127.8(4) . 10_556 ?
O3 Rb4A U2 74.16(19) . . ?
O3 Rb4A P3A 24.8(3) . . ?
O3 Rb4A P3B 23.0(2) . . ?
O3 Rb4A O6A 63.6(7) . 10_556 ?
O6A Rb4A U2 33.9(6) 10_556 . ?
O6A Rb4A U2 32.4(7) . . ?
O6A Rb4A P3A 59.5(7) 10_556 . ?
O6A Rb4A P3A 23.6(7) . . ?
O6A Rb4A P3B 56.3(7) 10_556 . ?
O6A Rb4A P3B 23.3(8) . . ?
O6A Rb4A O2 95.1(9) . . ?
O6A Rb4A O3 45.2(8) . . ?
O6A Rb4A O6A 45.1(12) . 10_556 ?
O6A Rb4A O6B 6.7(10) . . ?
O6A Rb4A O8 53.9(8) . . ?
O6A Rb4A O8 58.3(8) . 10_556 ?
O6B Rb4A U2 36.7(6) . . ?
O6B Rb4A P3A 21.5(6) . . ?
O6B Rb4A P3B 22.2(6) . . ?
O6B Rb4A O3 45.2(6) . . ?
O6B Rb4A O6A 51.8(5) . 10_556 ?
O6B Rb4A O8 61.8(6) . 10_556 ?
O8 Rb4A U2 26.3(3) 10_556 . ?
O8 Rb4A U2 25.2(3) . . ?
O8 Rb4A P3A 81.9(4) 10_556 . ?
O8 Rb4A P3A 77.2(4) . . ?
O8 Rb4A P3B 81.1(3) 10_556 . ?
O8 Rb4A P3B 77.2(4) . . ?
O8 Rb4A O3 98.4(3) . . ?
O8 Rb4A O3 100.0(3) 10_556 . ?
O8 Rb4A O6A 53.5(7) . 10_556 ?
O8 Rb4A O6A 46.5(7) 10_556 10_556 ?
O8 Rb4A O6B 56.0(6) . . ?
O8 Rb4A O8 12.1(6) . 10_556 ?
Rb4A Rb4B U2 88.1(19) . . ?
Rb4A Rb4B U2 88.1(19) 10_556 . ?
Rb4A Rb4B Rb4A 169(4) . 10_556 ?
Rb4A Rb4B P3A 54.8(19) . . ?
Rb4A Rb4B P3A 115(2) 10_556 . ?
Rb4A Rb4B P3A 54.8(19) 10_556 10_556 ?
Rb4A Rb4B P3A 115(2) . 10_556 ?
Rb4A Rb4B O2 86.1(17) 10_556 . ?
Rb4A Rb4B O2 86.1(17) . . ?
Rb4A Rb4B O6A 110(2) 10_556 . ?
Rb4A Rb4B O6A 110(2) . 10_556 ?
Rb4A Rb4B O6A 62(2) . . ?
Rb4A Rb4B O6A 62(2) 10_556 10_556 ?
Rb4A Rb4B O6B 58.1(19) . . ?
Rb4A Rb4B O6B 114(2) . 10_556 ?
Rb4A Rb4B O6B 114(2) 10_556 . ?
Rb4A Rb4B O6B 58.1(19) 10_556 10_556 ?
Rb4A Rb4B O8 97.0(18) 10_556 . ?
Rb4A Rb4B O8 97.0(18) . 10_556 ?
Rb4A Rb4B O8 84.0(17) . . ?
Rb4A Rb4B O8 84.0(17) 10_556 10_556 ?
P3A Rb4B U2 53.6(4) 10_556 . ?
P3A Rb4B U2 53.6(4) . . ?
P3A Rb4B P3A 60.1(6) 10_556 . ?
O2 Rb4B U2 116.1(9) . . ?
O2 Rb4B P3A 72.3(6) . 10_556 ?
O2 Rb4B P3A 72.3(6) . . ?
O2 Rb4B O6A 90.4(10) . 10_556 ?
O2 Rb4B O6A 90.4(10) . . ?
O2 Rb4B O6B 90.8(9) . . ?
O2 Rb4B O6B 90.8(9) . 10_556 ?
O2 Rb4B O8 140.8(11) . . ?
O2 Rb4B O8 140.8(11) . 10_556 ?
O6A Rb4B U2 34.3(7) . . ?
O6A Rb4B U2 34.3(7) 10_556 . ?
O6A Rb4B P3A 19.8(7) 10_556 10_556 ?
O6A Rb4B P3A 57.4(8) 10_556 . ?
O6A Rb4B P3A 19.8(7) . . ?
O6A Rb4B P3A 57.4(8) . 10_556 ?
O6A Rb4B O6A 47.4(13) . 10_556 ?
O6A Rb4B O6B 51.7(6) . 10_556 ?
O6A Rb4B O6B 4.3(10) 10_556 10_556 ?
O6A Rb4B O6B 4.3(10) . . ?
O6A Rb4B O6B 51.7(6) 10_556 . ?
O6B Rb4B U2 36.9(6) . . ?
O6B Rb4B U2 37.0(6) 10_556 . ?
O6B Rb4B P3A 18.9(6) . . ?
O6B Rb4B P3A 61.6(7) 10_556 . ?
O6B Rb4B P3A 18.9(6) 10_556 10_556 ?
O6B Rb4B P3A 61.6(7) . 10_556 ?
O6B Rb4B O6B 56.0(11) . 10_556 ?
O8 Rb4B U2 25.9(4) . . ?
O8 Rb4B U2 25.9(4) 10_556 . ?
O8 Rb4B P3A 71.0(6) 10_556 10_556 ?
O8 Rb4B P3A 71.0(6) . . ?
O8 Rb4B P3A 77.8(6) 10_556 . ?
O8 Rb4B P3A 77.8(6) . 10_556 ?
O8 Rb4B O6A 51.6(8) 10_556 10_556 ?
O8 Rb4B O6A 51.6(8) . . ?
O8 Rb4B O6A 58.0(9) 10_556 . ?
O8 Rb4B O6A 58.0(9) . 10_556 ?
O8 Rb4B O6B 52.1(7) 10_556 10_556 ?
O8 Rb4B O6B 59.5(7) . 10_556 ?
O8 Rb4B O6B 52.1(7) . . ?
O8 Rb4B O6B 59.5(7) 10_556 . ?
O8 Rb4B O8 13.0(6) . 10_556 ?
Rb5B Rb5A Rb5B 58(3) 7_456 . ?
Rb5B Rb5A Rb5C 29.2(15) 7_456 . ?
Rb5B Rb5A Rb5C 29.2(15) . . ?
Rb5B Rb5A O1 87.6(18) . 7_456 ?
Rb5B Rb5A O1 82.4(17) . . ?
Rb5B Rb5A O1 87.6(18) 7_456 . ?
Rb5B Rb5A O1 82.4(17) 7_456 7_456 ?
Rb5B Rb5A O11A 109.4(12) 7_456 5_556 ?
Rb5B Rb5A O11A 66.5(12) . 5_556 ?
Rb5B Rb5A O11A 109.4(12) . 4_565 ?
Rb5B Rb5A O11A 66.5(13) 7_456 4_565 ?
Rb5B Rb5A O11B 114.1(13) 7_456 5_556 ?
Rb5B Rb5A O11B 74.8(13) . 5_556 ?
Rb5B Rb5A O14 96.0(17) 7_456 11_567 ?
Rb5B Rb5A O14 96.0(17) . 5_556 ?
Rb5B Rb5A O14 148.1(19) 7_456 5_556 ?
Rb5B Rb5A O14 148.1(19) . 11_567 ?
Rb5B Rb5A O17 19.8(18) 7_456 7_456 ?
Rb5B Rb5A O17 19.8(18) . . ?
Rb5B Rb5A O17 66.3(18) . 7_456 ?
Rb5B Rb5A O17 66.3(18) 7_456 . ?
Rb5C Rb5A O1 84.3(2) . . ?
Rb5C Rb5A O1 84.3(2) . 7_456 ?
Rb5C Rb5A O11A 87.8(4) . 5_556 ?
Rb5C Rb5A O11A 87.8(4) . 4_565 ?
Rb5C Rb5A O11B 94.8(4) . 5_556 ?
Rb5C Rb5A O14 123.12(19) . 11_567 ?
Rb5C Rb5A O14 123.12(19) . 5_556 ?
Rb5C Rb5A O17 39.7(3) . . ?
Rb5C Rb5A O17 39.7(3) . 7_456 ?
O1 Rb5A O1 168.6(5) 7_456 . ?
O1 Rb5A O11A 53.8(4) . 4_565 ?
O1 Rb5A O11A 53.8(4) 7_456 5_556 ?
O1 Rb5A O11A 125.6(4) . 5_556 ?
O1 Rb5A O11A 125.6(4) 7_456 4_565 ?
O1 Rb5A O11B 131.2(3) . 5_556 ?
O1 Rb5A O11B 50.0(3) 7_456 5_556 ?
O1 Rb5A O14 68.9(2) . 5_556 ?
O1 Rb5A O14 118.0(3) . 11_567 ?
O1 Rb5A O14 68.9(2) 7_456 11_567 ?
O1 Rb5A O14 118.0(3) 7_456 5_556 ?
O1 Rb5A O17 107.1(4) 7_456 . ?
O1 Rb5A O17 63.5(4) . . ?
O1 Rb5A O17 107.1(4) . 7_456 ?
O1 Rb5A O17 63.5(4) 7_456 7_456 ?
O11A Rb5A O11A 175.6(7) 5_556 4_565 ?
O11A Rb5A O11B 8.5(3) 5_556 5_556 ?
O11A Rb5A O11B 174.5(5) 4_565 5_556 ?
O14 Rb5A O11A 71.3(4) 5_556 5_556 ?
O14 Rb5A O11A 111.2(4) 11_567 5_556 ?
O14 Rb5A O11A 111.2(4) 5_556 4_565 ?
O14 Rb5A O11A 71.3(4) 11_567 4_565 ?
O14 Rb5A O11B 71.4(4) 5_556 5_556 ?
O14 Rb5A O11B 103.2(4) 11_567 5_556 ?
O14 Rb5A O14 113.8(4) 11_567 5_556 ?
O17 Rb5A O11A 76.7(5) . 5_556 ?
O17 Rb5A O11A 99.8(5) . 4_565 ?
O17 Rb5A O11A 76.7(4) 7_456 4_565 ?
O17 Rb5A O11A 99.8(5) 7_456 5_556 ?
O17 Rb5A O11B 102.3(5) 7_456 5_556 ?
O17 Rb5A O11B 85.2(4) . 5_556 ?
O17 Rb5A O14 83.6(4) . 5_556 ?
O17 Rb5A O14 162.3(4) . 11_567 ?
O17 Rb5A O14 83.6(4) 7_456 11_567 ?
O17 Rb5A O14 162.3(4) 7_456 5_556 ?
O17 Rb5A O17 79.4(6) 7_456 . ?
Rb5A Rb5B O1 77(2) . 7_456 ?
Rb5A Rb5B O1 81.6(13) . . ?
Rb5A Rb5B O3 130(2) . 16_566 ?
Rb5A Rb5B O11A 100.4(15) . 5_556 ?
Rb5A Rb5B O11B 92.3(14) . 5_556 ?
Rb5A Rb5B O14 69.7(13) . 5_556 ?
Rb5A Rb5B O17 138(2) . 10_556 ?
Rb5A Rb5B O17 153(2) . . ?
Rb5A Rb5B O17 98(2) . 7_456 ?
Rb5B Rb5B Rb5A 60.8(15) 7_456 . ?
Rb5B Rb5B O1 77(4) 7_456 7_456 ?
Rb5B Rb5B O1 88(3) 7_456 . ?
Rb5B Rb5B O3 111(3) 7_456 16_566 ?
Rb5B Rb5B O11A 133(4) 7_456 5_556 ?
Rb5B Rb5B O11B 127(4) 7_456 5_556 ?
Rb5B Rb5B O14 126.7(12) 7_456 5_556 ?
Rb5B Rb5B O17 130(3) 7_456 10_556 ?
Rb5B Rb5B O17 124.0(18) 7_456 . ?
Rb5B Rb5B O17 42(2) 7_456 7_456 ?
Rb5C Rb5B Rb5A 100(8) . . ?
Rb5C Rb5B Rb5B 40(7) . 7_456 ?
Rb5C Rb5B O1 85(4) . 7_456 ?
Rb5C Rb5B O1 93(2) . . ?
Rb5C Rb5B O3 86(3) . 16_566 ?
Rb5C Rb5B O11A 130(2) . 5_556 ?
Rb5C Rb5B O11B 130(2) . 5_556 ?
Rb5C Rb5B O14 158(3) . 5_556 ?
Rb5C Rb5B O17 20(3) . 7_456 ?
Rb5C Rb5B O17 100(7) . 10_556 ?
Rb5C Rb5B O17 89(7) . . ?
O1 Rb5B O1 157.5(13) . 7_456 ?
O1 Rb5B O3 54.4(4) 7_456 16_566 ?
O1 Rb5B O3 148.1(13) . 16_566 ?
O1 Rb5B O11A 56.1(5) 7_456 5_556 ?
O1 Rb5B O11A 135.0(10) . 5_556 ?
O1 Rb5B O11B 51.2(5) 7_456 5_556 ?
O1 Rb5B O11B 136.3(8) . 5_556 ?
O1 Rb5B O14 66.2(5) . 5_556 ?
O1 Rb5B O14 110.3(7) 7_456 5_556 ?
O1 Rb5B O17 141.0(9) 7_456 10_556 ?
O1 Rb5B O17 61.4(7) . 10_556 ?
O3 Rb5B O11B 50.6(4) 16_566 5_556 ?
O11A Rb5B O3 45.8(5) 5_556 16_566 ?
O11A Rb5B O11B 8.3(4) 5_556 5_556 ?
O14 Rb5B O3 115.1(6) 5_556 16_566 ?
O14 Rb5B O11A 72.4(6) 5_556 5_556 ?
O14 Rb5B O11B 71.0(5) 5_556 5_556 ?
O17 Rb5B O1 72.5(9) . . ?
O17 Rb5B O1 113.2(7) 7_456 . ?
O17 Rb5B O1 65.1(7) 7_456 7_456 ?
O17 Rb5B O1 129.8(9) . 7_456 ?
O17 Rb5B O3 72.4(5) 7_456 16_566 ?
O17 Rb5B O3 87.2(8) 10_556 16_566 ?
O17 Rb5B O3 75.6(8) . 16_566 ?
O17 Rb5B O11A 93.9(9) 10_556 5_556 ?
O17 Rb5B O11A 111.1(8) 7_456 5_556 ?
O17 Rb5B O11A 92.8(10) . 5_556 ?
O17 Rb5B O11B 110.5(8) 7_456 5_556 ?
O17 Rb5B O11B 101.0(10) . 5_556 ?
O17 Rb5B O11B 101.4(9) 10_556 5_556 ?
O17 Rb5B O14 92.5(11) . 5_556 ?
O17 Rb5B O14 78.0(8) 10_556 5_556 ?
O17 Rb5B O14 167.5(14) 7_456 5_556 ?
O17 Rb5B O17 15.6(5) . 10_556 ?
O17 Rb5B O17 99.3(10) . 7_456 ?
O17 Rb5B O17 113.2(10) 7_456 10_556 ?
Rb5A Rb5C O1 75.5(7) . . ?
Rb5A Rb5C O1 75.5(7) . 7_456 ?
Rb5A Rb5C O4A 157.9(4) . 10_556 ?
Rb5A Rb5C O4B 151.7(5) . 10_556 ?
Rb5A Rb5C O4B 151.7(5) . 16_566 ?
Rb5A Rb5C O17 123.0(9) . . ?
Rb5A Rb5C O17 123.0(9) . 7_456 ?
Rb5A Rb5C O17 112.2(7) . 10_556 ?
Rb5A Rb5C O17 112.2(7) . 16_566 ?
Rb5B Rb5C Rb5A 50(7) 7_456 . ?
Rb5B Rb5C Rb5A 50(7) . . ?
Rb5B Rb5C Rb5B 101(10) 7_456 . ?
Rb5B Rb5C O1 85(4) . 7_456 ?
Rb5B Rb5C O1 85(4) 7_456 . ?
Rb5B Rb5C O1 77(2) 7_456 7_456 ?
Rb5B Rb5C O1 77(2) . . ?
Rb5B Rb5C O4A 136(7) . 10_556 ?
Rb5B Rb5C O4A 118(5) 7_456 10_556 ?
Rb5B Rb5C O4B 123(7) . 10_556 ?
Rb5B Rb5C O4B 123(7) 7_456 16_566 ?
Rb5B Rb5C O4B 125(5) . 16_566 ?
Rb5B Rb5C O4B 125(5) 7_456 10_556 ?
Rb5B Rb5C O17 144(4) . 16_566 ?
Rb5B Rb5C O17 71(6) 7_456 16_566 ?
Rb5B Rb5C O17 71(6) . 10_556 ?
Rb5B Rb5C O17 78(6) . . ?
Rb5B Rb5C O17 144(4) 7_456 10_556 ?
Rb5B Rb5C O17 78(6) 7_456 7_456 ?
Rb5B Rb5C O17 155(3) . 7_456 ?
Rb5B Rb5C O17 155(3) 7_456 . ?
O1 Rb5C O1 151.0(14) 7_456 . ?
O1 Rb5C O4A 122.9(9) 7_456 10_556 ?
O1 Rb5C O4A 85.5(6) . 10_556 ?
O1 Rb5C O4B 132.8(11) 7_456 10_556 ?
O1 Rb5C O4B 76.2(6) 7_456 16_566 ?
O1 Rb5C O4B 76.2(6) . 10_556 ?
O1 Rb5C O4B 132.8(11) . 16_566 ?
O1 Rb5C O17 134.7(4) 7_456 10_556 ?
O1 Rb5C O17 134.6(4) . 16_566 ?
O1 Rb5C O17 59.1(3) . 10_556 ?
O1 Rb5C O17 59.1(3) 7_456 16_566 ?
O4B Rb5C O4A 13.5(4) 10_556 10_556 ?
O4B Rb5C O4A 48.7(7) 16_566 10_556 ?
O4B Rb5C O4B 56.6(9) 10_556 16_566 ?
O17 Rb5C O1 127.5(6) . 7_456 ?
O17 Rb5C O1 70.4(4) 7_456 7_456 ?
O17 Rb5C O1 70.4(4) . . ?
O17 Rb5C O1 127.5(6) 7_456 . ?
O17 Rb5C O4A 73.7(8) 16_566 10_556 ?
O17 Rb5C O4A 65.2(7) 10_556 10_556 ?
O17 Rb5C O4A 61.2(9) 7_456 10_556 ?
O17 Rb5C O4A 58.1(9) . 10_556 ?
O17 Rb5C O4B 87.1(9) 10_556 16_566 ?
O17 Rb5C O4B 45.9(8) 7_456 16_566 ?
O17 Rb5C O4B 45.9(8) . 10_556 ?
O17 Rb5C O4B 52.1(6) 16_566 16_566 ?
O17 Rb5C O4B 74.7(11) . 16_566 ?
O17 Rb5C O4B 52.1(6) 10_556 10_556 ?
O17 Rb5C O4B 87.1(9) 16_566 10_556 ?
O17 Rb5C O4B 74.7(11) 7_456 10_556 ?
O17 Rb5C O17 12.6(4) 7_456 16_566 ?
O17 Rb5C O17 12.6(4) . 10_556 ?
O17 Rb5C O17 124.4(15) 7_456 10_556 ?
O17 Rb5C O17 135.7(14) 10_556 16_566 ?
O17 Rb5C O17 113.9(18) 7_456 . ?
O17 Rb5C O17 124.4(15) . 16_566 ?
O2 Rb6 O6B 112.0(5) 3_654 10 ?
O2 Rb6 O9A 76.2(4) 3_654 . ?
O2 Rb6 O9A 76.2(4) 3_654 10 ?
O2 Rb6 O16 148.5(3) 3_654 7_455 ?
O2 Rb6 O16 148.5(3) 3_654 16_565 ?
O5A Rb6 O2 142.7(3) 10 3_654 ?
O5A Rb6 O2 142.7(3) . 3_654 ?
O5A Rb6 O5A 51.5(5) . 10 ?
O5A Rb6 O6B 92.0(6) . 10 ?
O5A Rb6 O6B 40.6(6) 10 10 ?
O5A Rb6 O9A 90.2(4) . . ?
O5A Rb6 O9A 138.9(5) 10 . ?
O5A Rb6 O9A 90.2(4) 10 10 ?
O5A Rb6 O9A 138.9(5) . 10 ?
O5A Rb6 O9B 132.4(4) . 10 ?
O5A Rb6 O9B 88.7(4) . . ?
O5A Rb6 O9B 88.7(4) 10 10 ?
O5A Rb6 O9B 132.4(4) 10 . ?
O5A Rb6 O10A 132.8(4) 10 10 ?
O5A Rb6 O10A 132.7(4) . . ?
O5A Rb6 O10A 148.3(4) 10 . ?
O5A Rb6 O10A 148.3(4) . 10 ?
O5A Rb6 O16 59.8(4) . 16_565 ?
O5A Rb6 O16 65.2(4) . 7_455 ?
O5A Rb6 O16 65.2(4) 10 16_565 ?
O5A Rb6 O16 59.8(4) 10 7_455 ?
O9A Rb6 O6B 50.8(6) 10 10 ?
O9A Rb6 O6B 161.0(7) . 10 ?
O9A Rb6 O9A 119.2(8) . 10 ?
O9B Rb6 O2 84.5(3) . 3_654 ?
O9B Rb6 O2 84.5(3) 10 3_654 ?
O9B Rb6 O6B 149.0(7) . 10 ?
O9B Rb6 O6B 52.6(6) 10 10 ?
O9B Rb6 O9A 113.8(5) 10 . ?
O9B Rb6 O9A 12.3(4) . . ?
O9B Rb6 O9A 12.3(4) 10 10 ?
O9B Rb6 O9A 113.8(5) . 10 ?
O9B Rb6 O9B 106.4(7) 10 . ?
O9B Rb6 O16 72.7(4) . 16_565 ?
O9B Rb6 O16 81.6(4) 10 16_565 ?
O9B Rb6 O16 72.7(4) 10 7_455 ?
O9B Rb6 O16 81.6(4) . 7_455 ?
O10A Rb6 O2 58.7(3) 10 3_654 ?
O10A Rb6 O2 58.7(3) . 3_654 ?
O10A Rb6 O6B 98.0(6) 10 10 ?
O10A Rb6 O6B 120.1(6) . 10 ?
O10A Rb6 O9A 48.2(4) 10 10 ?
O10A Rb6 O9A 71.1(4) . 10 ?
O10A Rb6 O9A 48.2(4) . . ?
O10A Rb6 O9A 71.1(4) 10 . ?
O10A Rb6 O9B 67.5(4) . 10 ?
O10A Rb6 O9B 45.6(4) . . ?
O10A Rb6 O9B 67.5(4) 10 . ?
O10A Rb6 O9B 45.6(4) 10 10 ?
O10A Rb6 O10A 22.9(5) . 10 ?
O10A Rb6 O16 92.1(3) . 7_455 ?
O10A Rb6 O16 89.9(3) . 16_565 ?
O10A Rb6 O16 89.9(3) 10 7_455 ?
O10A Rb6 O16 92.1(3) 10 16_565 ?
O16 Rb6 O6B 81.0(6) 16_565 10 ?
O16 Rb6 O6B 70.8(6) 7_455 10 ?
O16 Rb6 O9A 83.9(5) 7_455 10 ?
O16 Rb6 O9A 93.3(5) 7_455 . ?
O16 Rb6 O9A 83.9(5) 16_565 . ?
O16 Rb6 O9A 93.3(5) 16_565 10 ?
O16 Rb6 O16 10.9(5) 16_565 7_455 ?
Rb1 P1 Rb1 97.65(3) 7_455 15_666 ?
Rb1 P1 Rb1 111.26(4) 7_455 9_565 ?
Rb1 P1 Rb1 97.66(3) 9_565 . ?
Rb1 P1 Rb1 120.27(4) 9_565 15_666 ?
Rb1 P1 Rb1 111.26(4) 15_666 . ?
Rb1 P1 Rb1 120.27(4) 7_455 . ?
O15A P1 Rb1 85.5(8) . . ?
O15A P1 Rb1 85.5(8) 8 15_666 ?
O15A P1 Rb1 65.1(10) 8 . ?
O15A P1 Rb1 171.6(9) 8 7_455 ?
O15A P1 Rb1 60.7(8) 2_565 15_666 ?
O15A P1 Rb1 65.1(10) 2_565 7_455 ?
O15A P1 Rb1 171.6(9) 2_565 . ?
O15A P1 Rb1 60.7(8) . 7_455 ?
O15A P1 Rb1 171.6(9) 7_455 15_666 ?
O15A P1 Rb1 60.7(8) 8 9_565 ?
O15A P1 Rb1 65.1(10) . 15_666 ?
O15A P1 Rb1 65.1(10) 7_455 9_565 ?
O15A P1 Rb1 60.7(8) 7_455 . ?
O15A P1 Rb1 85.5(8) 2_565 9_565 ?
O15A P1 Rb1 171.6(9) . 9_565 ?
O15A P1 Rb1 85.5(8) 7_455 7_455 ?
O15A P1 O15A 92.4(16) 8 7_455 ?
O15A P1 O15A 127.5(16) 7_455 2_565 ?
O15A P1 O15A 110(2) 8 2_565 ?
O15A P1 O15A 110(2) 7_455 . ?
O15A P1 O15A 92.4(16) 2_565 . ?
O15A P1 O15A 127.5(16) 8 . ?
O15A P1 O15B 19.2(10) 8 8 ?
O15A P1 O15B 107.3(12) . 2_565 ?
O15A P1 O15B 19.2(10) 2_565 2_565 ?
O15A P1 O15B 19.2(10) . . ?
O15A P1 O15B 109.6(12) . 8 ?
O15A P1 O15B 19.2(10) 7_455 7_455 ?
O15A P1 O15B 107.3(12) 7_455 8 ?
O15A P1 O15B 108.1(10) 8 2_565 ?
O15A P1 O15B 108.1(10) 7_455 . ?
O15A P1 O15B 108.1(10) 2_565 8 ?
O15A P1 O15B 107.3(12) 2_565 . ?
O15A P1 O15B 109.6(12) 7_455 2_565 ?
O15A P1 O15B 109.6(12) 2_565 7_455 ?
O15A P1 O15B 108.1(10) . 7_455 ?
O15A P1 O15B 109.6(12) 8 . ?
O15A P1 O15B 107.3(12) 8 7_455 ?
O15B P1 Rb1 78.7(10) 2_565 15_666 ?
O15B P1 Rb1 69.1(9) . . ?
O15B P1 Rb1 166.5(8) . 9_565 ?
O15B P1 Rb1 166.5(8) 7_455 15_666 ?
O15B P1 Rb1 78.7(10) 7_455 . ?
O15B P1 Rb1 78.7(10) 8 9_565 ?
O15B P1 Rb1 69.1(9) 8 15_666 ?
O15B P1 Rb1 69.1(9) 2_565 9_565 ?
O15B P1 Rb1 65.2(14) 8 . ?
O15B P1 Rb1 65.2(14) 7_455 9_565 ?
O15B P1 Rb1 69.1(9) 7_455 7_455 ?
O15B P1 Rb1 78.7(10) . 7_455 ?
O15B P1 Rb1 65.2(14) . 15_666 ?
O15B P1 Rb1 166.5(8) 8 7_455 ?
O15B P1 Rb1 65.2(14) 2_565 7_455 ?
O15B P1 Rb1 166.5(8) 2_565 . ?
O15B P1 O15B 113(3) . 7_455 ?
O15B P1 O15B 113(3) 8 2_565 ?
O15B P1 O15B 124.3(18) . 2_565 ?
O15B P1 O15B 124.3(18) 8 7_455 ?
O15B P1 O15B 93(2) . 8 ?
O15B P1 O15B 93(2) 2_565 7_455 ?
U1 P2A Rb1 77.45(18) 3_654 . ?
U1 P2A Rb6 74.4(2) 3_654 . ?
Rb1 P2A Rb6 101.0(2) . . ?
P2B P2A U1 156.7(9) . 3_654 ?
P2B P2A Rb1 101.7(8) . . ?
P2B P2A Rb6 127.9(9) . . ?
P2B P2A O9A 72.9(12) . . ?
P2B P2A O9B 74.0(10) . . ?
P2B P2A O10A 145.0(11) . . ?
P2B P2A O10B 26.5(8) . . ?
P2B P2A O11A 108.2(13) . . ?
P2B P2A O11B 119.7(16) . . ?
P2B P2A O12A 45.8(15) . . ?
P2B P2A O12B 51.1(12) . . ?
O9A P2A U1 122.0(9) . 3_654 ?
O9A P2A Rb1 142.1(10) . . ?
O9A P2A Rb6 60.7(9) . . ?
O9A P2A O9B 25.8(8) . . ?
O9A P2A O10A 110.7(11) . . ?
O9A P2A O10B 67.3(10) . . ?
O9A P2A O11A 109.9(14) . . ?
O9A P2A O12A 113.6(16) . . ?
O9A P2A O12B 110.9(13) . . ?
O9B P2A U1 127.7(7) . 3_654 ?
O9B P2A Rb1 116.4(7) . . ?
O9B P2A Rb6 53.9(7) . . ?
O9B P2A O10B 80.1(9) . . ?
O9B P2A O12B 94.6(11) . . ?
O10A P2A U1 51.5(6) . 3_654 ?
O10A P2A Rb1 53.1(5) . . ?
O10A P2A Rb6 51.5(5) . . ?
O10A P2A O9B 94.8(9) . . ?
O10A P2A O10B 171.1(7) . . ?
O10A P2A O12B 98.5(11) . . ?
O10B P2A U1 137.2(4) . 3_654 ?
O10B P2A Rb1 122.8(4) . . ?
O10B P2A Rb6 127.9(4) . . ?
O11A P2A U1 51.6(9) . 3_654 ?
O11A P2A Rb1 107.3(10) . . ?
O11A P2A Rb6 108.7(10) . . ?
O11A P2A O9B 135.0(12) . . ?
O11A P2A O10A 103.1(12) . . ?
O11A P2A O10B 85.6(10) . . ?
O11A P2A O12A 111.1(15) . . ?
O11A P2A O12B 122.5(13) . . ?
O11B P2A U1 38.5(12) . 3_654 ?
O11B P2A Rb1 95.4(13) . . ?
O11B P2A Rb6 104.0(14) . . ?
O11B P2A O9A 120.2(17) . . ?
O11B P2A O9B 143.0(15) . . ?
O11B P2A O10A 89.4(15) . . ?
O11B P2A O10B 99.0(12) . . ?
O11B P2A O11A 14.5(15) . . ?
O11B P2A O12A 111.8(18) . . ?
O11B P2A O12B 121.2(17) . . ?
O12A P2A U1 124.4(13) . 3_654 ?
O12A P2A Rb1 56.8(13) . . ?
O12A P2A Rb6 138.7(11) . . ?
O12A P2A O9B 101.8(14) . . ?
O12A P2A O10A 107.9(14) . . ?
O12A P2A O10B 66.5(14) . . ?
O12A P2A O12B 12.7(16) . . ?
O12B P2A U1 125.2(10) . 3_654 ?
O12B P2A Rb1 50.8(10) . . ?
O12B P2A Rb6 126.2(9) . . ?
O12B P2A O10B 74.9(11) . . ?
U2 P2B Rb2 75.60(15) . . ?
U3 P2B U2 91.1(3) . . ?
U3 P2B Rb2 80.2(2) . . ?
P2A P2B U2 118.4(9) . . ?
P2A P2B U3 150.1(9) . . ?
P2A P2B Rb2 110.0(8) . . ?
P2A P2B O9A 82.0(12) . . ?
P2A P2B O9B 82.2(11) . . ?
P2A P2B O10A 25.0(8) . . ?
P2A P2B O10B 143.2(11) . . ?
P2A P2B O11A 52.1(11) . . ?
P2A P2B O11B 38.3(11) . . ?
P2A P2B O12A 111.8(19) . . ?
P2A P2B O12B 109.6(14) . . ?
O9A P2B U2 38.1(9) . . ?
O9A P2B U3 127.8(10) . . ?
O9A P2B Rb2 76.3(10) . . ?
O9A P2B O9B 26.6(9) . . ?
O9A P2B O10A 87.8(11) . . ?
O9A P2B O10B 86.5(11) . . ?
O9A P2B O11A 97.4(13) . . ?
O9A P2B O11B 99.0(14) . . ?
O9A P2B O12B 136.5(15) . . ?
O9B P2B U2 52.0(8) . . ?
O9B P2B U3 123.3(7) . . ?
O9B P2B Rb2 52.6(6) . . ?
O9B P2B O10A 76.6(9) . . ?
O9B P2B O10B 102.3(9) . . ?
O9B P2B O11A 116.6(11) . . ?
O10A P2B U2 125.4(4) . . ?
O10A P2B U3 137.3(4) . . ?
O10A P2B Rb2 87.9(4) . . ?
O10B P2B U2 50.8(4) . . ?
O10B P2B U3 53.3(5) . . ?
O10B P2B Rb2 101.0(6) . . ?
O10B P2B O10A 167.9(7) . . ?
O10B P2B O11A 95.3(9) . . ?
O11A P2B U2 110.0(8) . . ?
O11A P2B U3 116.0(8) . . ?
O11A P2B Rb2 162.0(9) . . ?
O11A P2B O10A 74.9(9) . . ?
O11B P2B U2 120.2(9) . . ?
O11B P2B U3 123.9(10) . . ?
O11B P2B Rb2 147.7(10) . . ?
O11B P2B O9B 112.3(12) . . ?
O11B P2B O10A 59.8(10) . . ?
O11B P2B O10B 110.7(9) . . ?
O11B P2B O11A 15.4(10) . . ?
O11B P2B O12B 116.3(15) . . ?
O12A P2B U2 127.4(17) . . ?
O12A P2B U3 42.4(17) . . ?
O12A P2B Rb2 73.7(14) . . ?
O12A P2B O9A 149.7(18) . . ?
O12A P2B O9B 125.5(16) . . ?
O12A P2B O10A 94.9(18) . . ?
O12A P2B O10B 95.4(18) . . ?
O12A P2B O11A 112.4(17) . . ?
O12A P2B O11B 108.4(19) . . ?
O12A P2B O12B 15(2) . . ?
O12B P2B U2 123.1(12) . . ?
O12B P2B U3 49.9(11) . . ?
O12B P2B Rb2 60.2(10) . . ?
O12B P2B O9B 111.2(13) . . ?
O12B P2B O10A 88.7(12) . . ?
O12B P2B O10B 102.8(13) . . ?
O12B P2B O11A 123.3(13) . . ?
U4 P3A Rb3 71.2(3) 16_565 11_566 ?
U4 P3A Rb4A 150.1(5) 16_565 . ?
U4 P3A Rb4B 161.3(5) 16_565 . ?
U4 P3A Rb6 69.1(3) 16_565 . ?
Rb3 P3A Rb4B 96.5(4) 11_566 . ?
Rb3 P3A Rb6 76.0(3) 11_566 . ?
Rb4A P3A Rb3 87.3(3) . 11_566 ?
Rb4A P3A Rb4B 11.3(3) . . ?
Rb4A P3A Rb6 86.0(3) . . ?
Rb6 P3A Rb4B 94.7(4) . . ?
O3 P3A U4 115.5(8) . 16_565 ?
O3 P3A Rb3 69.1(6) . 11_566 ?
O3 P3A Rb4A 73.1(7) . . ?
O3 P3A Rb4B 70.6(7) . . ?
O3 P3A Rb6 139.7(8) . . ?
O3 P3A O4A 109.9(10) . . ?
O3 P3A O4B 92.8(9) . . ?
O3 P3A O5A 109.9(10) . . ?
O3 P3A O5B 109.0(11) . . ?
O4A P3A U4 53.6(9) . 16_565 ?
O4A P3A Rb3 118.5(9) . 11_566 ?
O4A P3A Rb4A 153.8(9) . . ?
O4A P3A Rb4B 143.2(9) . . ?
O4A P3A Rb6 104.0(9) . . ?
O4A P3A O4B 23.8(7) . . ?
O4B P3A U4 75.5(8) . 16_565 ?
O4B P3A Rb3 128.8(7) . 11_566 ?
O4B P3A Rb4A 134.1(8) . . ?
O4B P3A Rb4B 122.8(8) . . ?
O4B P3A Rb6 125.4(9) . . ?
O5A P3A U4 49.0(6) . 16_565 ?
O5A P3A Rb3 40.9(6) . 11_566 ?
O5A P3A Rb4A 101.3(7) . . ?
O5A P3A Rb4B 112.6(7) . . ?
O5A P3A Rb6 40.3(6) . . ?
O5A P3A O4A 101.9(12) . . ?
O5A P3A O4B 124.4(11) . . ?
O5A P3A O5B 35.7(8) . . ?
O5B P3A U4 15.4(6) . 16_565 ?
O5B P3A Rb3 56.3(7) . 11_566 ?
O5B P3A Rb4A 136.4(8) . . ?
O5B P3A Rb4B 147.7(8) . . ?
O5B P3A Rb6 64.1(8) . . ?
O5B P3A O4A 68.6(11) . . ?
O5B P3A O4B 89.4(10) . . ?
O6A P3A U4 134.4(13) . 16_565 ?
O6A P3A Rb3 129.0(16) . 11_566 ?
O6A P3A Rb4A 48.3(13) . . ?
O6A P3A Rb4B 44.2(12) . . ?
O6A P3A Rb6 77.0(15) . . ?
O6A P3A O3 110.1(14) . . ?
O6A P3A O4A 109.6(17) . . ?
O6A P3A O4B 102.1(17) . . ?
O6A P3A O5A 115.1(18) . . ?
O6A P3A O5B 138.4(17) . . ?
O6B P3A U4 115.4(14) . 16_565 ?
O6B P3A Rb3 127.5(16) . 11_566 ?
O6B P3A Rb4A 61.9(14) . . ?
O6B P3A Rb4B 60.6(14) . . ?
O6B P3A Rb6 61.4(14) . . ?
O6B P3A O3 129.1(15) . . ?
O6B P3A O4A 101.3(18) . . ?
O6B P3A O4B 101.6(18) . . ?
O6B P3A O5A 101.4(17) . . ?
O6B P3A O5B 119.6(17) . . ?
O6B P3A O6A 19.2(16) . . ?
U4 P3B U4 81.9(3) 16_565 10_556 ?
U4 P3B Rb4A 138.3(5) 16_565 . ?
U4 P3B Rb4A 139.2(4) 10_556 . ?
U4 P3B Rb5B 70.4(4) 10_556 16_565 ?
U4 P3B Rb5B 66.4(6) 16_565 16_565 ?
U4 P3B Rb5C 62.8(4) 10_556 10_556 ?
U4 P3B Rb5C 65.9(3) 16_565 10_556 ?
Rb5B P3B Rb4A 124.6(5) 16_565 . ?
Rb5C P3B Rb4A 130.4(5) 10_556 . ?
Rb5C P3B Rb5B 7.6(3) 10_556 16_565 ?
O3 P3B U4 110.1(7) . 10_556 ?
O3 P3B U4 122.3(7) . 16_565 ?
O3 P3B Rb4A 59.9(6) . . ?
O3 P3B Rb5B 66.0(7) . 16_565 ?
O3 P3B Rb5C 70.9(7) . 10_556 ?
O3 P3B O5A 97.1(9) . . ?
O3 P3B O6A 95.8(12) . . ?
O3 P3B O6B 109.2(13) . . ?
O4A P3B U4 57.5(11) . 16_565 ?
O4A P3B U4 29.7(9) . 10_556 ?
O4A P3B Rb4A 154.5(11) . . ?
O4A P3B Rb5B 77.9(10) . 16_565 ?
O4A P3B Rb5C 71.0(10) . 10_556 ?
O4A P3B O3 135.8(13) . . ?
O4A P3B O4B 32.1(10) . . ?
O4A P3B O5A 109.1(13) . . ?
O4A P3B O5B 80.8(13) . . ?
O4A P3B O6A 116.8(16) . . ?
O4A P3B O6B 109.0(17) . . ?
O4B P3B U4 5.7(7) . 10_556 ?
O4B P3B U4 86.5(10) . 16_565 ?
O4B P3B Rb4A 134.1(9) . . ?
O4B P3B Rb5B 75.4(9) . 16_565 ?
O4B P3B Rb5C 67.9(8) . 10_556 ?
O4B P3B O3 110.6(11) . . ?
O4B P3B O5A 140.5(12) . . ?
O4B P3B O5B 109.6(12) . . ?
O4B P3B O6A 110.7(15) . . ?
O4B P3B O6B 112.2(16) . . ?
O5A P3B U4 136.3(7) . 10_556 ?
O5A P3B U4 54.5(5) . 16_565 ?
O5A P3B Rb4A 83.9(6) . . ?
O5A P3B Rb5B 91.8(8) . 16_565 ?
O5A P3B Rb5C 97.2(6) . 10_556 ?
O5B P3B U4 23.4(6) . 16_565 ?
O5B P3B U4 104.8(8) . 10_556 ?
O5B P3B Rb4A 116.0(8) . . ?
O5B P3B Rb5B 70.5(10) . 16_565 ?
O5B P3B Rb5C 73.2(8) . 10_556 ?
O5B P3B O3 108.4(11) . . ?
O5B P3B O5A 32.4(7) . . ?
O5B P3B O6A 120.7(15) . . ?
O5B P3B O6B 106.7(15) . . ?
O6A P3B U4 116.3(13) . 10_556 ?
O6A P3B U4 130.0(12) . 16_565 ?
O6A P3B Rb4A 38.8(11) . . ?
O6A P3B Rb5B 161.6(12) . 16_565 ?
O6A P3B Rb5C 164.0(12) . 10_556 ?
O6A P3B O5A 93.2(14) . . ?
O6B P3B U4 114.0(12) . 16_565 ?
O6B P3B U4 117.2(14) . 10_556 ?
O6B P3B Rb4A 49.6(11) . . ?
O6B P3B Rb5B 172.3(14) . 16_565 ?
O6B P3B Rb5C 179.9(14) . 10_556 ?
O6B P3B O5A 82.7(13) . . ?
O6B P3B O6A 16.1(13) . . ?
U1 O1 Rb1 106.2(4) . 11_566 ?
U1 O1 Rb5A 125.62(17) . . ?
U1 O1 Rb5A 125.62(17) . 10_556 ?
U1 O1 Rb5B 113.5(6) . 7_456 ?
U1 O1 Rb5B 127.2(5) . . ?
U1 O1 Rb5B 127.2(5) . 10_556 ?
U1 O1 Rb5B 113.5(6) . 16_565 ?
U1 O1 Rb5C 117.4(4) . 10_556 ?
U1 O1 Rb5C 117.4(4) . . ?
Rb5A O1 Rb1 85.2(3) . 11_566 ?
Rb5A O1 Rb1 85.2(3) 10_556 11_566 ?
Rb5A O1 Rb5A 107.9(3) 10_556 . ?
Rb5A O1 Rb5B 116.9(6) . 16_565 ?
Rb5A O1 Rb5B 16.0(6) . . ?
Rb5A O1 Rb5B 15.8(5) . 7_456 ?
Rb5A O1 Rb5B 16.0(6) 10_556 10_556 ?
Rb5A O1 Rb5B 15.8(5) 10_556 16_565 ?
Rb5A O1 Rb5B 101.5(7) 10_556 . ?
Rb5A O1 Rb5B 116.9(6) 10_556 7_456 ?
Rb5A O1 Rb5B 101.5(7) . 10_556 ?
Rb5A O1 Rb5C 20.2(8) 10_556 10_556 ?
Rb5A O1 Rb5C 20.2(8) . . ?
Rb5A O1 Rb5C 109.5(3) . 10_556 ?
Rb5A O1 Rb5C 109.5(3) 10_556 . ?
Rb5B O1 Rb1 99.4(6) 10_556 11_566 ?
Rb5B O1 Rb1 99.4(6) . 11_566 ?
Rb5B O1 Rb1 98.8(5) 16_565 11_566 ?
Rb5B O1 Rb1 98.8(5) 7_456 11_566 ?
Rb5B O1 Rb5B 15.4(11) . 7_456 ?
Rb5B O1 Rb5B 91.7(13) 10_556 . ?
Rb5B O1 Rb5B 106.9(4) 10_556 7_456 ?
Rb5B O1 Rb5B 15.4(11) 10_556 16_565 ?
Rb5B O1 Rb5B 122.0(10) 16_565 7_456 ?
Rb5B O1 Rb5B 106.9(4) . 16_565 ?
Rb5B O1 Rb5C 113.0(6) 7_456 10_556 ?
Rb5B O1 Rb5C 9.9(4) . . ?
Rb5B O1 Rb5C 9.9(5) 7_456 . ?
Rb5B O1 Rb5C 9.9(4) 10_556 10_556 ?
Rb5B O1 Rb5C 113.0(6) 16_565 . ?
Rb5B O1 Rb5C 98.3(6) . 10_556 ?
Rb5B O1 Rb5C 9.9(5) 16_565 10_556 ?
Rb5B O1 Rb5C 98.3(6) 10_556 . ?
Rb5C O1 Rb1 105.5(7) . 11_566 ?
Rb5C O1 Rb1 105.4(7) 10_556 11_566 ?
Rb5C O1 Rb5C 103.8(5) 10_556 . ?
U1 O2 Rb4A 121.6(5) . . ?
U1 O2 Rb4A 121.6(5) . 10_556 ?
U1 O2 Rb4B 124.4(8) . . ?
U1 O2 Rb6 114.0(5) . 11_566 ?
Rb4A O2 Rb4A 33.6(4) . 10_556 ?
Rb4A O2 Rb6 121.2(4) . 11_566 ?
Rb4A O2 Rb6 121.2(4) 10_556 11_566 ?
Rb4B O2 Rb4A 16.85(19) . 10_556 ?
Rb4B O2 Rb4A 16.85(19) . . ?
Rb4B O2 Rb6 121.5(7) . 11_566 ?
U1 O3 Rb3 109.3(3) . 11_566 ?
U1 O3 Rb4A 91.6(3) . . ?
U1 O3 Rb5B 87.3(6) . 16_565 ?
U1 O3 Rb5C 89.6(5) . 10_556 ?
Rb4A O3 Rb3 93.3(3) . 11_566 ?
Rb4A O3 Rb5B 165.7(5) . 16_565 ?
Rb4A O3 Rb5C 173.8(4) . 10_556 ?
Rb5B O3 Rb3 73.7(5) 16_565 11_566 ?
Rb5B O3 Rb5C 8.5(4) 16_565 10_556 ?
Rb5C O3 Rb3 80.6(3) 10_556 11_566 ?
P3A O3 U1 162.2(8) . . ?
P3A O3 Rb3 87.7(6) . 11_566 ?
P3A O3 Rb4A 82.0(7) . . ?
P3A O3 Rb5B 102.9(9) . 16_565 ?
P3A O3 Rb5C 98.6(9) . 10_556 ?
P3A O3 P3B 17.2(4) . . ?
P3B O3 U1 153.5(8) . . ?
P3B O3 Rb3 95.2(6) . 11_566 ?
P3B O3 Rb4A 97.0(6) . . ?
P3B O3 Rb5B 90.2(8) . 16_565 ?
P3B O3 Rb5C 84.6(8) . 10_556 ?
U4 O4A U4 127.6(5) 16_565 . ?
U4 O4A U4 13.15(14) 10_556 . ?
U4 O4A U4 114.4(6) 10_556 16_565 ?
U4 O4A Rb5C 74.7(4) 10_556 10_556 ?
U4 O4A Rb5C 80.2(4) . 10_556 ?
U4 O4A Rb5C 73.2(4) 16_565 10_556 ?
P3A O4A U4 143.6(12) . 10_556 ?
P3A O4A U4 132.0(11) . . ?
P3A O4A U4 96.2(10) . 16_565 ?
P3A O4A Rb5C 97.3(8) . 10_556 ?
P3A O4A O5B 55.1(9) . . ?
P3B O4A U4 99.5(12) . 16_565 ?
P3B O4A U4 136.1(14) . 10_556 ?
P3B O4A U4 125.4(13) . . ?
P3B O4A Rb5C 90.5(11) . 10_556 ?
P3B O4A P3A 8.8(10) . . ?
P3B O4A O5B 58.3(10) . . ?
O4B O4A U4 27.3(16) . . ?
O4B O4A U4 39.0(15) . 10_556 ?
O4B O4A U4 146.5(19) . 16_565 ?
O4B O4A Rb5C 78.4(18) . 10_556 ?
O4B O4A P3A 105(2) . . ?
O4B O4A P3B 98(2) . . ?
O4B O4A O5B 146(2) . . ?
O5B O4A U4 157.8(10) . . ?
O5B O4A U4 148.5(10) . 10_556 ?
O5B O4A U4 41.2(7) . 16_565 ?
O5B O4A Rb5C 77.8(8) . 10_556 ?
U4 O4B U4 20.2(3) 10_556 . ?
U4 O4B Rb5C 82.8(6) 10_556 10_556 ?
U4 O4B Rb5C 92.2(6) . 10_556 ?
U4 O4B P3A 174.0(11) 10_556 . ?
P3A O4B U4 164.9(11) . . ?
P3A O4B Rb5C 92.4(8) . 10_556 ?
P3B O4B U4 167.1(14) . . ?
P3B O4B U4 169.5(12) . 10_556 ?
P3B O4B Rb5C 87.9(9) . 10_556 ?
P3B O4B P3A 4.7(8) . . ?
O4A O4B U4 125(2) . 10_556 ?
O4A O4B U4 143(2) . . ?
O4A O4B Rb5C 88.1(17) . 10_556 ?
O4A O4B P3A 51.4(17) . . ?
O4A O4B P3B 49.7(17) . . ?
U4 O5A U4 16.51(10) 16_565 7_455 ?
U4 O5A Rb3 101.9(5) 16_565 11_566 ?
U4 O5A Rb3 92.7(4) 7_455 11_566 ?
U4 O5A Rb6 90.1(4) 7_455 . ?
U4 O5A Rb6 98.9(4) 16_565 . ?
Rb6 O5A Rb3 112.7(5) . 11_566 ?
P3A O5A U4 102.0(7) . 16_565 ?
P3A O5A U4 118.5(8) . 7_455 ?
P3A O5A Rb3 117.9(8) . 11_566 ?
P3A O5A Rb6 118.8(9) . . ?
P3A O5A P3B 13.7(5) . . ?
P3B O5A U4 88.5(6) . 16_565 ?
P3B O5A U4 105.0(7) . 7_455 ?
P3B O5A Rb3 119.2(7) . 11_566 ?
P3B O5A Rb6 124.6(8) . . ?
O5B O5A U4 47.2(11) . 7_455 ?
O5B O5A U4 31.5(10) . 16_565 ?
O5B O5A Rb3 105.6(15) . 11_566 ?
O5B O5A Rb6 123.3(14) . . ?
O5B O5A P3A 72.6(12) . . ?
O5B O5A P3B 58.9(11) . . ?
U4 O5B U4 17.72(19) 16_565 7_455 ?
U4 O5B Rb3 94.3(5) 7_455 11_566 ?
U4 O5B Rb3 108.7(7) 16_565 11_566 ?
U4 O5B Rb5B 88.8(7) 7_455 16_565 ?
U4 O5B Rb5B 82.6(8) 16_565 16_565 ?
U4 O5B Rb5C 88.7(6) 7_455 10_556 ?
U4 O5B Rb5C 80.2(7) 16_565 10_556 ?
U4 O5B Rb6 96.2(7) 16_565 . ?
U4 O5B Rb6 85.9(5) 7_455 . ?
U4 O5B O4A 94.6(10) 16_565 . ?
Rb3 O5B Rb5B 76.3(5) 11_566 16_565 ?
Rb3 O5B Rb5C 84.5(6) 11_566 10_556 ?
Rb3 O5B Rb6 89.8(4) 11_566 . ?
Rb5C O5B Rb5B 8.2(3) 10_556 16_565 ?
Rb6 O5B Rb5B 164.7(7) . 16_565 ?
Rb6 O5B Rb5C 171.8(6) . 10_556 ?
P3A O5B U4 165.6(12) . 7_455 ?
P3A O5B U4 150.3(12) . 16_565 ?
P3A O5B Rb3 99.9(8) . 11_566 ?
P3A O5B Rb5B 96.8(10) . 16_565 ?
P3A O5B Rb5C 95.0(8) . 10_556 ?
P3A O5B Rb6 91.7(9) . . ?
P3A O5B O4A 56.3(9) . . ?
P3B O5B U4 152.9(10) . 7_455 ?
P3B O5B U4 135.3(11) . 16_565 ?
P3B O5B Rb3 110.2(9) . 11_566 ?
P3B O5B Rb5B 86.2(10) . 16_565 ?
P3B O5B Rb5C 82.7(8) . 10_556 ?
P3B O5B Rb6 104.8(9) . . ?
P3B O5B P3A 17.0(4) . . ?
P3B O5B O4A 40.8(9) . . ?
O4A O5B U4 112.1(10) . 7_455 ?
O4A O5B Rb3 144.5(10) . 11_566 ?
O4A O5B Rb5B 80.8(9) . 16_565 ?
O4A O5B Rb5C 73.3(8) . 10_556 ?
O4A O5B Rb6 114.5(10) . . ?
O5A O5B U4 114.9(13) . 7_455 ?
O5A O5B U4 131.1(15) . 16_565 ?
O5A O5B Rb3 57.7(13) . 11_566 ?
O5A O5B Rb5B 128.4(15) . 16_565 ?
O5A O5B Rb5C 135.4(16) . 10_556 ?
O5A O5B Rb6 43.3(12) . . ?
O5A O5B P3A 71.7(12) . . ?
O5A O5B P3B 88.7(13) . . ?
O5A O5B O4A 123.7(16) . . ?
U2 O6A Rb4A 106.3(10) . . ?
U2 O6A Rb4A 87.5(7) . 10_556 ?
U2 O6A Rb4B 95.4(9) . . ?
Rb4A O6A Rb4A 29.1(4) . 10_556 ?
Rb4A O6A Rb4B 15.7(3) . . ?
Rb4B O6A Rb4A 13.4(3) . 10_556 ?
P3A O6A U2 145(2) . . ?
P3A O6A Rb4A 108.0(18) . . ?
P3A O6A Rb4A 119.7(17) . 10_556 ?
P3A O6A Rb4B 116.0(18) . . ?
P3A O6A P3B 13.3(7) . . ?
P3B O6A U2 132.2(19) . . ?
P3B O6A Rb4A 123.5(16) . 10_556 ?
P3B O6A Rb4A 118.0(17) . . ?
P3B O6A Rb4B 123.1(17) . . ?
U2 O6B Rb4A 92.3(9) . . ?
U2 O6B Rb4B 82.1(8) . . ?
U2 O6B Rb6 110.9(11) . . ?
Rb4A O6B Rb4B 13.3(3) . . ?
Rb4A O6B Rb6 100.4(9) . . ?
Rb6 O6B Rb4B 112.0(10) . . ?
P3A O6B U2 147(2) . . ?
P3A O6B Rb4A 96.6(16) . . ?
P3A O6B Rb4B 100.5(16) . . ?
P3A O6B Rb6 98.9(15) . . ?
P3A O6B P3B 15.2(8) . . ?
P3B O6B U2 133.6(19) . . ?
P3B O6B Rb4A 108.2(15) . . ?
P3B O6B Rb4B 109.5(15) . . ?
P3B O6B Rb6 105.7(13) . . ?
U2 O7 Rb2 124.6(2) . 10_556 ?
U2 O7 Rb2 124.6(2) . . ?
Rb2 O7 Rb2 103.2(3) . 10_556 ?
U2 O8 Rb3 113.5(6) . . ?
U2 O8 Rb4A 110.5(5) . . ?
U2 O8 Rb4A 103.4(5) . 10_556 ?
U2 O8 Rb4B 109.0(7) . . ?
Rb3 O8 Rb4A 128.0(5) . 10_556 ?
Rb4A O8 Rb3 135.7(5) . . ?
Rb4A O8 Rb4A 31.5(3) . 10_556 ?
Rb4B O8 Rb3 132.1(7) . . ?
Rb4B O8 Rb4A 16.3(2) . . ?
Rb4B O8 Rb4A 15.33(19) . 10_556 ?
O8 O8 U2 79.4(5) 10_556 . ?
O8 O8 Rb3 83.7(3) 10_556 . ?
O8 O8 Rb4A 99.7(4) 10_556 . ?
O8 O8 Rb4A 68.2(3) 10_556 10_556 ?
O8 O8 Rb4B 83.5(3) 10_556 . ?
U2 O9A Rb6 122.8(8) . . ?
P2A O9A U2 142.0(14) . . ?
P2A O9A Rb6 95.2(10) . . ?
P2B O9A U2 118.4(13) . . ?
P2B O9A Rb6 117.8(12) . . ?
P2B O9A P2A 25.1(4) . . ?
O9B O9A U2 110(3) . . ?
O9B O9A Rb6 68(2) . . ?
O9B O9A P2A 83(3) . . ?
O9B O9A P2B 83(3) . . ?
U2 O9B Rb2 98.6(5) . . ?
U2 O9B Rb6 118.9(6) . . ?
Rb6 O9B Rb2 106.4(6) . . ?
P2A O9B U2 116.3(10) . . ?
P2A O9B Rb2 115.9(8) . . ?
P2A O9B Rb6 101.1(8) . . ?
P2B O9B U2 99.9(10) . . ?
P2B O9B Rb2 104.3(8) . . ?
P2B O9B Rb6 124.9(9) . . ?
P2B O9B P2A 23.8(3) . . ?
O9A O9B U2 56(2) . . ?
O9A O9B Rb2 150(3) . . ?
O9A O9B Rb6 100(3) . . ?
O9A O9B P2A 71(2) . . ?
O9A O9B P2B 70(2) . . ?
U1 O10A Rb1 102.3(4) 3_654 . ?
U1 O10A Rb6 98.7(4) 3_654 . ?
Rb1 O10A Rb6 143.9(5) . . ?
P2A O10A U1 98.2(7) . 3_654 ?
P2A O10A Rb1 101.6(6) . . ?
P2A O10A Rb6 104.0(6) . . ?
P2A O10A P2B 10.0(3) . . ?
P2B O10A U1 107.2(6) . 3_654 ?
P2B O10A Rb1 95.3(5) . . ?
P2B O10A Rb6 106.1(5) . . ?
O10A O10A U1 76.1(3) 10 3_654 ?
O10A O10A Rb1 78.5(2) 10 . ?
O10A O10A Rb6 78.6(2) 10 . ?
O10A O10A P2A 174.1(6) 10 . ?
O10A O10A P2B 173.6(4) 10 . ?
U2 O10B Rb3 96.5(4) . . ?
U3 O10B U2 127.6(5) . . ?
U3 O10B Rb3 126.8(4) . . ?
P2A O10B U2 98.9(5) . . ?
P2A O10B U3 104.4(5) . . ?
P2A O10B Rb3 95.0(4) . . ?
P2B O10B U2 99.8(6) . . ?
P2B O10B U3 96.1(6) . . ?
P2B O10B Rb3 105.1(6) . . ?
P2B O10B P2A 10.4(3) . . ?
O10B O10B U2 79.5(3) 10_556 . ?
O10B O10B U3 79.5(2) 10_556 . ?
O10B O10B Rb3 81.4(2) 10_556 . ?
O10B O10B P2A 175.8(4) 10_556 . ?
O10B O10B P2B 173.6(5) 10_556 . ?
U1 O11A Rb3 131.7(8) 3_654 . ?
U1 O11A Rb5A 88.4(7) 3_654 3_654 ?
U1 O11A Rb5B 89.3(8) 3_654 5_546 ?
U1 O11A Rb5C 83.7(6) 3_654 3_654 ?
Rb3 O11A Rb5A 97.0(6) . 3_654 ?
Rb3 O11A Rb5B 86.7(9) . 5_546 ?
Rb3 O11A Rb5C 88.3(6) . 3_654 ?
Rb5A O11A Rb5C 16.5(6) 3_654 3_654 ?
Rb5B O11A Rb5A 13.1(5) 5_546 3_654 ?
Rb5B O11A Rb5C 6.3(4) 5_546 3_654 ?
P2A O11A U1 99.6(12) . 3_654 ?
P2A O11A Rb3 123.1(12) . . ?
P2A O11A Rb5A 108.9(11) . 3_654 ?
P2A O11A Rb5B 121.6(13) . 5_546 ?
P2A O11A Rb5C 125.3(13) . 3_654 ?
P2A O11A P2B 19.7(4) . . ?
P2B O11A U1 118.7(11) . 3_654 ?
P2B O11A Rb3 106.8(10) . . ?
P2B O11A Rb5A 102.9(9) . 3_654 ?
P2B O11A Rb5B 113.7(11) . 5_546 ?
P2B O11A Rb5C 119.0(11) . 3_654 ?
O11B O11A U1 73(4) . 3_654 ?
O11B O11A Rb3 152(4) . . ?
O11B O11A Rb5A 97(5) . 3_654 ?
O11B O11A Rb5B 110(5) . 5_546 ?
O11B O11A Rb5C 110(5) . 3_654 ?
O11B O11A P2A 29(3) . . ?
O11B O11A P2B 46(4) . . ?
U1 O11B Rb3 115.4(8) 3_654 . ?
U1 O11B Rb5A 87.5(6) 3_654 3_654 ?
U1 O11B Rb5B 85.8(7) 3_654 5_546 ?
Rb3 O11B Rb5A 86.8(5) . 3_654 ?
Rb3 O11B Rb5B 76.1(8) . 5_546 ?
Rb5B O11B Rb5A 12.9(5) 5_546 3_654 ?
P2A O11B U1 125.1(16) . 3_654 ?
P2A O11B Rb3 113.1(14) . . ?
P2A O11B Rb5A 119.6(16) . 3_654 ?
P2A O11B Rb5B 130.3(16) . 5_546 ?
P2A O11B P2B 22.0(6) . . ?
P2B O11B U1 146.5(13) . 3_654 ?
P2B O11B Rb3 95.9(9) . . ?
P2B O11B Rb5A 106.8(11) . 3_654 ?
P2B O11B Rb5B 114.6(12) . 5_546 ?
O11A O11B U1 95(4) . 3_654 ?
O11A O11B Rb3 23(4) . . ?
O11A O11B Rb5A 74(4) . 3_654 ?
O11A O11B Rb5B 62(4) . 5_546 ?
O11A O11B P2A 136(5) . . ?
O11A O11B P2B 118(4) . . ?
U3 O12A Rb1 123.0(13) . . ?
U3 O12A Rb2 94.1(9) . . ?
Rb1 O12A Rb2 92.0(7) . . ?
P2A O12A U3 138.2(19) . . ?
P2A O12A Rb1 97.7(16) . . ?
P2A O12A Rb2 93.6(14) . . ?
P2B O12A U3 117(2) . . ?
P2B O12A Rb1 119(2) . . ?
P2B O12A Rb2 87.6(17) . . ?
P2B O12A P2A 22.4(7) . . ?
U3 O12B Rb1 129.7(12) . . ?
U3 O12B Rb2 101.5(9) . . ?
Rb1 O12B Rb2 103.4(8) . . ?
P2A O12B U3 118.7(14) . . ?
P2A O12B Rb1 99.1(11) . . ?
P2A O12B Rb2 99.9(11) . . ?
P2B O12B U3 101.5(15) . . ?
P2B O12B Rb1 118.2(14) . . ?
P2B O12B Rb2 96.2(13) . . ?
P2B O12B P2A 19.3(4) . . ?
U3 O13 Rb1 109.1(5) . 7_455 ?
U3 O13 Rb2 123.8(3) . . ?
U3 O13 Rb2 123.8(3) . 10_556 ?
Rb1 O13 Rb2 100.3(2) 7_455 . ?
Rb1 O13 Rb2 100.3(2) 7_455 10_556 ?
Rb2 O13 Rb2 95.3(3) 10_556 . ?
U3 O14 Rb1 105.0(4) . 15_666 ?
U3 O14 Rb5A 129.98(16) . 12_657 ?
U3 O14 Rb5A 129.98(16) . 3_654 ?
U3 O14 Rb5B 135.6(5) . 5_546 ?
U3 O14 Rb5B 135.6(5) . 14_655 ?
Rb1 O14 Rb5B 95.2(5) 15_666 5_546 ?
Rb1 O14 Rb5B 95.2(5) 15_666 14_655 ?
Rb5A O14 Rb1 84.9(2) 12_657 15_666 ?
Rb5A O14 Rb1 84.9(2) 3_654 15_666 ?
Rb5A O14 Rb5A 99.3(3) 3_654 12_657 ?
Rb5A O14 Rb5B 14.3(6) 3_654 5_546 ?
Rb5A O14 Rb5B 90.3(7) 12_657 5_546 ?
Rb5A O14 Rb5B 90.3(7) 3_654 14_655 ?
Rb5A O14 Rb5B 14.3(6) 12_657 14_655 ?
Rb5B O14 Rb5B 79.5(13) 5_546 14_655 ?
U3 O15A Rb1 91.2(8) . 15_666 ?
U3 O15A Rb1 94.3(8) . 7_455 ?
Rb1 O15A Rb1 115.4(6) 7_455 15_666 ?
P1 O15A U3 170.2(12) . . ?
P1 O15A Rb1 89.7(11) . 15_666 ?
P1 O15A Rb1 94.1(9) . 7_455 ?
O15B O15A U3 86(6) . . ?
O15B O15A Rb1 86(7) . 15_666 ?
O15B O15A Rb1 159(7) . 7_455 ?
O15B O15A P1 84(6) . . ?
U3 O15B Rb1 82.0(8) . 7_455 ?
U3 O15B Rb1 90.7(11) . 15_666 ?
U3 O15B Rb1 112.7(9) . . ?
Rb1 O15B Rb1 126.9(10) 15_666 . ?
Rb1 O15B Rb1 103.3(6) 15_666 7_455 ?
Rb1 O15B Rb1 125.9(12) . 7_455 ?
P1 O15B U3 157.5(14) . . ?
P1 O15B Rb1 76.2(10) . 7_455 ?
P1 O15B Rb1 88.9(15) . 15_666 ?
P1 O15B Rb1 85.1(11) . . ?
O15A O15B U3 81(6) . . ?
O15A O15B Rb1 18(6) . 7_455 ?
O15A O15B Rb1 143(7) . . ?
O15A O15B Rb1 85(7) . 15_666 ?
O15A O15B P1 76(6) . . ?
U4 O16 U4 25.57(18) . 10_556 ?
U4 O16 Rb2 146.1(6) 10_556 10_556 ?
U4 O16 Rb2 102.8(5) 10_556 . ?
U4 O16 Rb2 126.6(6) . . ?
U4 O16 Rb2 124.8(6) . 10_556 ?
U4 O16 Rb6 104.4(5) . 7_455 ?
U4 O16 Rb6 101.0(5) 10_556 7_455 ?
Rb2 O16 Rb2 94.2(3) 10_556 . ?
Rb2 O16 Rb6 106.1(4) 10_556 7_455 ?
Rb6 O16 Rb2 96.4(4) 7_455 . ?
O16 O16 U4 94.0(4) 10_556 . ?
O16 O16 U4 68.5(4) 10_556 10_556 ?
O16 O16 Rb2 39.3(2) 10_556 . ?
O16 O16 Rb2 133.5(3) 10_556 10_556 ?
O16 O16 Rb6 84.6(3) 10_556 7_455 ?
U4 O17 U4 23.9(2) . 10_556 ?
U4 O17 Rb3 98.4(6) . 5_556 ?
U4 O17 Rb3 93.3(5) 10_556 5_556 ?
U4 O17 Rb5A 145.8(8) . . ?
U4 O17 Rb5A 166.6(7) 10_556 . ?
U4 O17 Rb5B 163.6(10) 10_556 . ?
U4 O17 Rb5B 91.3(6) 10_556 10_556 ?
U4 O17 Rb5B 140.5(10) . . ?
U4 O17 Rb5B 130.4(11) . 7_456 ?
U4 O17 Rb5B 151.0(10) 10_556 7_456 ?
U4 O17 Rb5B 115.1(8) . 10_556 ?
U4 O17 Rb5C 128.6(11) . . ?
U4 O17 Rb5C 107.6(9) . 10_556 ?
U4 O17 Rb5C 150.5(11) 10_556 . ?
U4 O17 Rb5C 84.1(8) 10_556 10_556 ?
Rb5A O17 Rb3 98.5(4) . 5_556 ?
Rb5A O17 Rb5B 96.7(5) . 10_556 ?
Rb5A O17 Rb5C 102.7(7) . 10_556 ?
Rb5B O17 Rb3 81.1(5) 10_556 5_556 ?
Rb5B O17 Rb3 109.6(6) 7_456 5_556 ?
Rb5B O17 Rb3 96.4(7) . 5_556 ?
Rb5B O17 Rb5A 7.2(4) . . ?
Rb5B O17 Rb5A 15.9(7) 7_456 . ?
Rb5B O17 Rb5B 14.0(9) . 7_456 ?
Rb5B O17 Rb5B 109.2(10) 7_456 10_556 ?
Rb5B O17 Rb5B 103.2(9) . 10_556 ?
Rb5B O17 Rb5C 109.6(10) . 10_556 ?
Rb5B O17 Rb5C 13.3(7) . . ?
Rb5B O17 Rb5C 113.8(6) 7_456 10_556 ?
Rb5B O17 Rb5C 9.0(6) 10_556 10_556 ?
Rb5C O17 Rb3 106.7(7) . 5_556 ?
Rb5C O17 Rb3 87.0(4) 10_556 5_556 ?
Rb5C O17 Rb5A 17.3(8) . . ?
Rb5C O17 Rb5B 4.6(7) . 7_456 ?
Rb5C O17 Rb5B 112.6(9) . 10_556 ?
Rb5C O17 Rb5C 117.6(13) . 10_556 ?
O17 O17 U4 85.0(5) 10_556 . ?
O17 O17 U4 61.0(5) 10_556 10_556 ?
O17 O17 Rb3 80.1(3) 10_556 5_556 ?
O17 O17 Rb5A 127.2(3) 10_556 . ?
O17 O17 Rb5B 30.6(4) 10_556 10_556 ?
O17 O17 Rb5B 138.6(8) 10_556 7_456 ?
O17 O17 Rb5B 133.8(6) 10_556 . ?
O17 O17 Rb5C 24.9(6) 10_556 10_556 ?
O17 O17 Rb5C 142.5(8) 10_556 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 P2A 3.052(10) 4_565 ?
U1 P2A 3.052(10) 11_566 ?
U1 O1 1.810(10) . ?
U1 O2 1.787(10) . ?
U1 O3 2.270(8) . ?
U1 O3 2.270(8) 10_556 ?
U1 O10A 2.413(13) 11_566 ?
U1 O10A 2.413(13) 4_565 ?
U1 O11A 2.43(2) 4_565 ?
U1 O11A 2.43(2) 11_566 ?
U1 O11B 2.323(19) 11_566 ?
U1 O11B 2.323(19) 4_565 ?
U2 O6A 2.23(3) . ?
U2 O6A 2.23(3) 10_556 ?
U2 O6B 2.39(3) 10_556 ?
U2 O6B 2.39(3) . ?
U2 O7 1.766(10) . ?
U2 O8 1.822(14) 10_556 ?
U2 O8 1.822(14) . ?
U2 O9A 2.22(2) . ?
U2 O9A 2.22(2) 10_556 ?
U2 O9B 2.532(18) . ?
U2 O10B 2.490(11) . ?
U2 O10B 2.490(11) 10_556 ?
U3 O10B 2.483(12) 10_556 ?
U3 O10B 2.483(12) . ?
U3 O12A 2.34(3) 10_556 ?
U3 O12A 2.34(3) . ?
U3 O12B 2.41(3) 10_556 ?
U3 O12B 2.41(3) . ?
U3 O13 1.778(10) . ?
U3 O14 1.780(10) . ?
U3 O15A 2.26(3) 10_556 ?
U3 O15A 2.26(3) . ?
U3 O15B 2.28(3) 10_556 ?
U3 O15B 2.28(3) . ?
U4 U4 0.8370(12) 10_556 ?
U4 O4A 2.506(19) 16_566 ?
U4 O4A 2.359(17) 10_556 ?
U4 O4B 2.25(2) . ?
U4 O4B 1.803(19) 10_556 ?
U4 O5A 2.385(14) 16_566 ?
U4 O5B 1.656(15) 16_566 ?
U4 O5B 2.246(14) 7_455 ?
U4 O16 1.804(12) . ?
U4 O16 1.935(13) 10_556 ?
U4 O17 1.807(15) . ?
U4 O17 2.057(16) 10_556 ?
Rb1 O10A 2.919(12) . ?
Rb1 O10A 2.919(12) 10 ?
Rb1 O12A 3.02(3) . ?
Rb1 O12A 3.02(3) 10 ?
Rb1 O12B 2.80(3) . ?
Rb1 O12B 2.80(3) 10 ?
Rb1 O13 3.034(11) 7_455 ?
Rb1 O14 3.133(11) 15_665 ?
Rb1 O15A 3.12(2) 7_455 ?
Rb1 O15A 3.24(3) 8 ?
Rb1 O15A 3.12(2) 16_565 ?
Rb1 O15A 3.24(3) 15_665 ?
Rb2 O7 2.997(6) . ?
Rb2 O7 2.997(6) 7_455 ?
Rb2 O9B 3.062(17) . ?
Rb2 O9B 3.062(17) 7_455 ?
Rb2 O12B 3.26(3) . ?
Rb2 O12B 3.26(3) 7_455 ?
Rb2 O13 3.178(7) . ?
Rb2 O13 3.178(7) 7_455 ?
Rb2 O16 2.987(13) 16_565 ?
Rb2 O16 2.987(13) 10_556 ?
Rb2 O16 3.415(14) 7_455 ?
Rb2 O16 3.415(14) . ?
Rb3 O5A 2.790(13) 12_656 ?
Rb3 O5A 2.790(13) 3_655 ?
Rb3 O5B 3.177(17) 12_656 ?
Rb3 O5B 3.177(17) 3_655 ?
Rb3 O8 3.032(13) 10_556 ?
Rb3 O8 3.032(13) . ?
Rb3 O10B 3.006(11) 10_556 ?
Rb3 O10B 3.006(11) . ?
Rb3 O11A 2.80(2) . ?
Rb3 O11A 2.80(2) 10_556 ?
Rb3 O11B 3.29(2) 10_556 ?
Rb3 O11B 3.29(2) . ?
Rb4A Rb4A 1.678(18) 10_556 ?
Rb4A Rb4B 0.843(10) . ?
Rb4A P3A 3.507(16) . ?
Rb4A P3B 3.887(15) . ?
Rb4A O2 2.902(11) . ?
Rb4A O3 3.389(12) . ?
Rb4A O6A 2.75(3) . ?
Rb4A O6A 3.42(2) 10_556 ?
Rb4A O6B 3.11(3) . ?
Rb4A O8 3.166(14) 10_556 ?
Rb4A O8 2.983(14) . ?
Rb4B P3A 3.92(3) . ?
Rb4B P3A 3.92(3) 10_556 ?
Rb4B O2 2.83(2) . ?
Rb4B O6A 3.04(4) 10_556 ?
Rb4B O6A 3.04(4) . ?
Rb4B O6B 3.48(4) . ?
Rb4B O6B 3.48(4) 10_556 ?
Rb4B O8 2.95(3) . ?
Rb4B O8 2.95(3) 10_556 ?
Rb5A Rb5B 0.81(3) . ?
Rb5A Rb5B 0.81(3) 7_456 ?
Rb5A Rb5C 1.04(4) . ?
Rb5A O1 2.905(6) . ?
Rb5A O1 2.905(6) 7_456 ?
Rb5A O11A 3.52(2) 4_565 ?
Rb5A O11A 3.52(2) 5_556 ?
Rb5A O11B 3.63(2) 5_556 ?
Rb5A O14 3.083(7) 5_556 ?
Rb5A O14 3.083(7) 11_567 ?
Rb5A O17 2.929(16) 7_456 ?
Rb5A O17 2.929(16) . ?
Rb5B Rb5B 0.79(6) 7_456 ?
Rb5B Rb5C 0.51(2) . ?
Rb5B O1 2.98(3) 7_456 ?
Rb5B O1 2.91(2) . ?
Rb5B O3 3.475(19) 16_566 ?
Rb5B O11A 3.29(3) 5_556 ?
Rb5B O11B 3.51(3) 5_556 ?
Rb5B O14 3.269(19) 5_556 ?
Rb5B O17 3.10(4) 10_556 ?
Rb5B O17 2.18(4) . ?
Rb5B O17 2.71(3) 7_456 ?
Rb5C O1 2.986(11) 7_456 ?
Rb5C O1 2.986(11) . ?
Rb5C O4A 3.47(4) 10_556 ?
Rb5C O4B 3.40(4) 16_566 ?
Rb5C O4B 3.40(4) 10_556 ?
Rb5C O17 3.23(2) 10_556 ?
Rb5C O17 2.23(3) . ?
Rb5C O17 2.23(3) 7_456 ?
Rb5C O17 3.23(2) 16_566 ?
Rb6 O2 2.996(11) 3_654 ?
Rb6 O5A 2.786(13) . ?
Rb6 O5A 2.786(13) 10 ?
Rb6 O6B 3.35(3) 10 ?
Rb6 O9A 3.18(2) 10 ?
Rb6 O9A 3.18(2) . ?
Rb6 O9B 2.992(16) 10 ?
Rb6 O9B 2.992(16) . ?
Rb6 O10A 2.927(13) 10 ?
Rb6 O10A 2.927(13) . ?
Rb6 O16 3.080(13) 16_565 ?
Rb6 O16 3.080(13) 7_455 ?
P1 O15A 1.52(3) . ?
P1 O15A 1.52(3) 2_565 ?
P1 O15A 1.52(3) 7_455 ?
P1 O15A 1.52(3) 8 ?
P1 O15B 1.56(3) . ?
P1 O15B 1.56(3) 2_565 ?
P1 O15B 1.56(3) 8 ?
P1 O15B 1.56(3) 7_455 ?
P2A P2B 0.637(5) . ?
P2A O9A 1.49(2) . ?
P2A O9B 1.561(16) . ?
P2A O10A 1.556(15) . ?
P2A O10B 2.123(14) . ?
P2A O11A 1.49(2) . ?
P2A O11B 1.05(2) . ?
P2A O12A 1.55(3) . ?
P2A O12B 1.82(3) . ?
P2B O9A 1.44(2) . ?
P2B O9B 1.515(17) . ?
P2B O10A 2.110(15) . ?
P2B O10B 1.579(13) . ?
P2B O11A 1.80(2) . ?
P2B O11B 1.47(2) . ?
P2B O12A 1.20(3) . ?
P2B O12B 1.50(3) . ?
P3A O3 1.487(16) . ?
P3A O4A 1.565(18) . ?
P3A O4B 1.94(2) . ?
P3A O5A 1.536(18) . ?
P3A O5B 1.54(2) . ?
P3A O6A 1.48(3) . ?
P3A O6B 1.29(3) . ?
P3B O3 1.533(16) . ?
P3B O4A 1.16(2) . ?
P3B O4B 1.505(19) . ?
P3B O5A 1.763(17) . ?
P3B O5B 1.511(19) . ?
P3B O6A 1.74(4) . ?
P3B O6B 1.55(3) . ?
O4A O4B 0.81(2) . ?
O4A O5B 1.75(2) . ?
O5A O5B 0.944(18) . ?
O8 O8 0.67(3) 10_556 ?
O9A O9B 0.68(2) . ?
O10A O10A 1.16(2) 10 ?
O10B O10B 0.90(2) 10_556 ?
O11A O11B 0.541(19) . ?
O15A O15B 0.51(3) . ?
O16 O16 0.58(3) 10_556 ?
O17 O17 1.16(3) 10_556 ?
